# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_123
_database_code_depnum_ccdc_archive 'CCDC 1838047'
loop_
_audit_author_name
_audit_author_address
Tohtihaji.Bahti
;Chinese Academy of Sciences
China
;
_audit_update_record             
;
2019-02-18 deposited with the CCDC.	2019-04-16 downloaded from the CCDC.
;
_audit_creation_date             2019-02-01
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'B20 Cs12 O40 Zn4'
_chemical_formula_sum            'B20 Cs12 O40 Zn4'
_chemical_formula_weight         2712.60
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           9
_space_group_name_H-M_alt        'C 1 c 1'
_space_group_name_Hall           'C -2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'

_cell_length_a                   18.739(16)
_cell_length_b                   19.326(16)
_cell_length_c                   14.495(12)
_cell_angle_alpha                90
_cell_angle_beta                 109.520(10)
_cell_angle_gamma                90
_cell_volume                     4948(7)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    2806
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      23.09
_cell_measurement_theta_min      2.41
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    10.723
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5349
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   
'SADABS-2008/1 (Bruker,2008) was used for absorption correction. wR2(int) was 0.1268 before and 0.0559 after correction. The Ratio of minimum to maximum transmission is 0.7174. The λ/2 correction factor is 0.0015.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.642
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4800
_exptl_crystal_size_max          0.243
_exptl_crystal_size_mid          0.224
_exptl_crystal_size_min          0.189
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0432
_diffrn_reflns_av_unetI/netI     0.0886
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            14935
_diffrn_reflns_point_group_measured_fraction_full 0.831
_diffrn_reflns_point_group_measured_fraction_max 0.809
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.627
_diffrn_reflns_theta_min         2.306
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.632
_reflns_Friedel_fraction_full    0.663
_reflns_Friedel_fraction_max     0.627
_reflns_number_gt                7089
_reflns_number_total             9328
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v7.68A (Bruker, 2009)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v7.68A (Bruker, 2009)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         1.846
_refine_diff_density_min         -1.923
_refine_diff_density_rms         0.276
_refine_ls_abs_structure_details 
;
 Flack x determined using 2006 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.04(3)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     685
_refine_ls_number_reflns         9328
_refine_ls_number_restraints     20
_refine_ls_R_factor_all          0.0796
_refine_ls_R_factor_gt           0.0537
_refine_ls_restrained_S_all      1.017
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0351P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0941
_refine_ls_wR_factor_ref         0.1068
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(B12) \\sim Ueq, Uanis(B19) \\sim Ueq, Uanis(B20) \\sim Ueq: with sigma of
0.005 and sigma for terminal atoms of 0.01
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Cs1 Cs 0.91893(7) 0.45091(8) 0.38483(10) 0.0266(3) Uani 1 1 d . . . . .
Cs2 Cs 0.63329(11) 0.69601(9) 0.41250(11) 0.0440(4) Uani 1 1 d . . . . .
Cs3 Cs 0.26526(8) 0.47024(11) 0.70912(11) 0.0496(5) Uani 1 1 d . . . . .
Cs4 Cs 0.43915(12) 0.43518(11) 0.41215(14) 0.0633(6) Uani 1 1 d . . . . .
Cs5 Cs 0.75893(8) 0.57839(7) 0.23919(10) 0.0279(3) Uani 1 1 d . . . . .
Cs6 Cs 0.08183(8) 0.56597(8) 0.53100(10) 0.0310(4) Uani 1 1 d . . . . .
Cs7 Cs 0.18908(8) 0.69997(9) 0.41508(10) 0.0332(4) Uani 1 1 d . . . . .
Cs8 Cs 0.60077(8) 0.56499(9) 0.60181(11) 0.0355(4) Uani 1 1 d . . . . .
Cs9 Cs 0.85849(9) 0.32938(10) 0.56207(10) 0.0391(4) Uani 1 1 d . . . . .
Cs10 Cs 0.51896(9) 0.69247(9) 0.75082(12) 0.0380(4) Uani 1 1 d . . . . .
Cs11 Cs 0.50339(8) 0.16568(10) 0.72965(10) 0.0390(4) Uani 1 1 d . . . . .
Cs12 Cs 0.33384(9) 0.29141(9) 0.57081(11) 0.0391(4) Uani 1 1 d . . . . .
Zn1 Zn 0.66523(13) 0.06533(14) 0.89696(16) 0.0196(6) Uani 1 1 d . . . . .
Zn2 Zn 0.42777(14) 0.18501(14) 0.37427(16) 0.0237(6) Uani 1 1 d . . . . .
Zn3 Zn 0.76492(14) 0.32842(14) 0.26555(15) 0.0216(5) Uani 1 1 d . . . . .
Zn4 Zn 0.50312(14) 0.45271(14) 0.72776(17) 0.0230(6) Uani 1 1 d . . . . .
B1 B 0.5890(12) 0.1331(13) 1.0186(16) 0.021(5) Uani 1 1 d . . . . .
B2 B 0.7979(12) 0.5706(12) 0.6295(13) 0.017(5) Uani 1 1 d . . . . .
B3 B 0.8048(16) 0.2414(13) 0.7416(18) 0.031(6) Uani 1 1 d . . . . .
B4 B 0.5594(13) 0.2523(16) 0.5223(16) 0.029(6) Uani 1 1 d . . . . .
B5 B 0.5684(13) 0.1376(13) 0.1719(16) 0.023(5) Uani 1 1 d . . . . .
B6 B 0.7678(13) 0.5138(12) 0.4746(15) 0.021(5) Uani 1 1 d . . . . .
B7 B 0.5903(13) 0.0187(14) 0.2451(15) 0.024(5) Uani 1 1 d . . . . .
B8 B 0.6312(13) 0.5150(14) 0.3839(17) 0.028(6) Uani 1 1 d . . . . .
B9 B 0.2834(13) 0.5413(13) 0.4894(16) 0.021(5) Uani 1 1 d . . . . .
B10 B 0.6612(14) 0.2146(15) 0.1409(16) 0.029(6) Uani 1 1 d . . . . .
B11 B 0.6644(12) 0.2507(13) 0.6857(15) 0.019(5) Uani 1 1 d . . . . .
B12 B 0.3723(13) 0.6224(14) 0.4443(17) 0.027(5) Uani 1 1 d . U . . .
B13 B 0.8548(13) 0.6150(16) 0.5058(16) 0.030(6) Uani 1 1 d . . . . .
B14 B 0.7019(15) 0.4120(15) 0.3777(17) 0.028(6) Uani 1 1 d . . . . .
B15 B 0.4113(14) 0.5599(13) 0.5984(17) 0.024(5) Uani 1 1 d . . . . .
B16 B 0.5778(13) 0.3545(13) 0.6321(17) 0.023(5) Uani 1 1 d . . . . .
B17 B 0.7349(13) 0.1692(14) 0.8217(17) 0.029(6) Uani 1 1 d . . . . .
B18 B 0.4939(14) 0.0906(14) 0.2718(17) 0.026(6) Uani 1 1 d . . . . .
B19 B 0.4215(15) 0.3626(15) 0.8038(19) 0.034(6) Uani 1 1 d . U . . .
B20 B 0.8824(15) 0.2369(15) 0.3705(18) 0.034(6) Uani 1 1 d . U . . .
O1 O 0.8273(7) 0.5564(7) 0.4535(9) 0.022(3) Uani 1 1 d . . . . .
O2 O 0.6172(7) 0.1993(8) 0.1963(10) 0.027(3) Uani 1 1 d . . . . .
O3 O 0.6309(7) 0.3164(7) 0.7024(9) 0.025(3) Uani 1 1 d . . . . .
O4 O 0.2133(7) 0.5165(7) 0.4755(9) 0.022(3) Uani 1 1 d . . . . .
O5 O 0.3579(7) 0.6956(8) 0.4312(10) 0.028(3) Uani 1 1 d . . . . .
O6 O 0.6147(7) 0.2177(7) 0.5942(9) 0.025(3) Uani 1 1 d . . . . .
O7 O 0.6146(9) 0.0761(8) 0.2073(12) 0.042(4) Uani 1 1 d . . . . .
O8 O 0.6708(7) 0.2033(7) 0.7671(10) 0.025(3) Uani 1 1 d . . . . .
O9 O 0.7678(7) 0.4449(7) 0.4345(9) 0.023(3) Uani 1 1 d . . . . .
O10 O 0.5100(7) 0.1434(7) 0.2184(9) 0.020(3) Uani 1 1 d . . . . .
O11 O 0.7837(8) 0.5105(8) 0.5807(9) 0.028(3) Uani 1 1 d . . . . .
O12 O 0.5633(7) 0.5492(8) 0.3664(10) 0.031(4) Uani 1 1 d . . . . .
O13 O 0.7399(8) 0.2656(8) 0.6795(10) 0.031(4) Uani 1 1 d . . . . .
O14 O 0.6963(8) 0.5499(8) 0.4326(10) 0.032(4) Uani 1 1 d . . . . .
O15 O 0.7007(8) 0.3482(7) 0.3450(10) 0.030(4) Uani 1 1 d . . . . .
O16 O 0.5593(8) 0.4196(8) 0.6427(10) 0.033(4) Uani 1 1 d . . . . .
O17 O 0.4660(7) 0.5448(8) 0.6861(10) 0.031(4) Uani 1 1 d . . . . .
O18 O 0.8721(8) 0.2674(10) 0.7551(11) 0.044(5) Uani 1 1 d . . . . .
O19 O 0.3442(8) 0.5245(8) 0.5751(11) 0.034(4) Uani 1 1 d . . . . .
O20 O 0.5384(8) 0.3198(9) 0.5437(11) 0.036(4) Uani 1 1 d . . . . .
O21 O 0.5349(7) 0.1306(8) 0.0645(9) 0.026(3) Uani 1 1 d . . . . .
O22 O 0.7433(8) 0.1291(9) 0.8980(10) 0.041(4) Uani 1 1 d . . . . .
O23 O 0.8362(8) 0.6250(7) 0.5941(9) 0.025(3) Uani 1 1 d . . . . .
O24 O 0.8934(10) 0.6653(9) 0.4831(12) 0.050(5) Uani 1 1 d . . . . .
O25 O 0.4434(8) 0.0964(9) 0.3192(11) 0.039(4) Uani 1 1 d . . . . .
O26 O 0.7124(10) 0.2648(10) 0.1614(12) 0.055(5) Uani 1 1 d . . . . .
O27 O 0.4298(10) 0.7087(10) 0.3245(12) 0.052(5) Uani 1 1 d . . . . .
O28 O 0.8003(8) 0.1811(11) 0.7981(13) 0.058(6) Uani 1 1 d . . . . .
O29 O 0.4299(9) 0.3838(10) 0.7207(11) 0.052(5) Uani 1 1 d . . . . .
O30 O 0.6349(9) 0.4467(9) 0.3553(13) 0.049(5) Uani 1 1 d . . . . .
O31 O 0.6272(8) -0.0419(8) 0.2568(10) 0.031(4) Uani 1 1 d . . . . .
O32 O 0.2986(7) 0.5855(8) 0.4248(9) 0.031(4) Uani 1 1 d . . . . .
O33 O 0.8626(9) 0.3034(8) 0.3550(11) 0.040(4) Uani 1 1 d . . . . .
O34 O 0.4262(8) 0.6046(9) 0.5378(10) 0.041(4) Uani 1 1 d . . . . .
O35 O 0.5281(9) 0.0272(8) 0.2747(13) 0.042(5) Uani 1 1 d . . . . .
O36 O 0.4016(8) 0.5949(8) 0.3650(11) 0.035(4) Uani 1 1 d . . . . .
O37 O 0.7776(7) 0.5825(7) 0.7084(8) 0.024(3) Uani 1 1 d . . . . .
O38 O 0.5824(7) 0.0973(8) 0.9374(10) 0.032(4) Uani 1 1 d . . . . .
O39 O 0.6517(8) 0.1753(8) 0.0571(9) 0.029(4) Uani 1 1 d . . . . .
O40 O 0.5269(7) 0.2250(8) 0.4355(8) 0.027(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cs1 Zn3 3.686(3) . ?
Cs1 B1 3.53(2) 4_554 ?
Cs1 B2 3.66(2) 2_564 ?
Cs1 B18 3.67(3) 3 ?
Cs1 O1 3.040(13) . ?
Cs1 O9 3.149(12) . ?
Cs1 O21 3.193(13) 4 ?
Cs1 O25 3.053(16) 3 ?
Cs1 O33 3.019(15) . ?
Cs1 O35 3.329(14) 3 ?
Cs1 O37 3.073(12) 2_564 ?
Cs1 O38 3.046(13) 4_554 ?
Cs2 B1 3.85(2) 2_564 ?
Cs2 B8 3.52(3) . ?
Cs2 B10 3.61(2) 2_565 ?
Cs2 B11 3.67(2) 2_564 ?
Cs2 B17 3.72(3) 2_564 ?
Cs2 O3 3.040(13) 2_564 ?
Cs2 O8 3.117(14) 2_564 ?
Cs2 O12 3.104(15) . ?
Cs2 O14 3.036(14) . ?
Cs2 O26 3.495(18) 2_565 ?
Cs2 O27 3.602(18) . ?
Cs2 O39 3.196(15) 2_565 ?
Cs3 B7 3.49(2) 4_455 ?
Cs3 B9 3.59(2) . ?
Cs3 B12 3.78(2) 2_565 ?
Cs3 B19 3.48(3) . ?
Cs3 O4 3.318(13) . ?
Cs3 O7 2.953(14) 4_455 ?
Cs3 O19 2.997(14) . ?
Cs3 O29 3.463(19) . ?
Cs3 O31 3.207(14) 4_455 ?
Cs3 O32 3.166(14) 2_565 ?
Cs3 O36 3.059(15) 2_565 ?
Cs3 O39 3.763(16) 4_455 ?
Cs4 Cs10 4.016(3) 2_564 ?
Cs4 Zn4 3.926(4) 2_564 ?
Cs4 B12 3.91(3) . ?
Cs4 B15 3.78(2) . ?
Cs4 B16 3.72(2) . ?
Cs4 O12 3.425(15) . ?
Cs4 O16 3.361(15) . ?
Cs4 O17 3.498(14) 2_564 ?
Cs4 O20 3.113(15) . ?
Cs4 O28 3.419(17) 4_454 ?
Cs4 O34 3.794(18) . ?
Cs4 O36 3.189(15) . ?
Cs5 B2 3.48(2) 2_564 ?
Cs5 B3 3.58(3) 2_564 ?
Cs5 B6 3.58(2) . ?
Cs5 B16 3.48(2) 2_564 ?
Cs5 O1 2.968(13) . ?
Cs5 O3 3.053(14) 2_564 ?
Cs5 O11 3.026(13) 2_564 ?
Cs5 O13 3.123(16) 2_564 ?
Cs5 O14 3.427(15) . ?
Cs5 O16 3.530(15) 2_564 ?
Cs5 O25 3.277(15) 3 ?
Cs5 O37 3.177(15) 2_564 ?
Cs6 Zn2 3.795(4) 3_455 ?
Cs6 B4 3.62(3) 3_455 ?
Cs6 B7 3.47(2) 4_455 ?
Cs6 B18 3.59(2) 3_455 ?
Cs6 O4 2.991(12) . ?
Cs6 O6 3.072(14) 3_455 ?
Cs6 O7 3.660(18) 4_455 ?
Cs6 O25 3.343(17) 3_455 ?
Cs6 O31 3.130(14) 4_455 ?
Cs6 O35 3.588(18) 3_455 ?
Cs6 O38 3.436(17) 4_454 ?
Cs6 O40 3.387(15) 3_455 ?
Cs7 B4 3.44(2) 3_455 ?
Cs7 B5 3.70(2) 3_455 ?
Cs7 B9 3.52(3) . ?
Cs7 B12 3.64(2) . ?
Cs7 O2 3.003(14) 3_455 ?
Cs7 O4 3.644(15) . ?
Cs7 O5 3.094(13) . ?
Cs7 O6 3.350(13) 3_455 ?
Cs7 O7 3.734(19) 3_455 ?
Cs7 O15 3.071(14) 3_455 ?
Cs7 O32 2.988(15) . ?
Cs7 O40 3.188(13) 3_455 ?
Cs8 Zn4 3.691(3) . ?
Cs8 B2 3.58(2) . ?
Cs8 B8 3.53(2) . ?
Cs8 B15 3.54(2) . ?
Cs8 O11 3.696(14) . ?
Cs8 O12 3.260(14) . ?
Cs8 O14 3.498(15) . ?
Cs8 O16 3.027(16) . ?
Cs8 O17 3.176(14) . ?
Cs8 O30 3.520(18) 2_565 ?
Cs8 O34 3.181(15) . ?
Cs8 O37 3.172(12) . ?
Cs9 B3 3.52(2) . ?
Cs9 B14 3.61(3) . ?
Cs9 B18 3.59(2) 4 ?
Cs9 B20 3.46(3) . ?
Cs9 O5 3.205(15) 3_545 ?
Cs9 O9 3.032(14) . ?
Cs9 O10 3.029(12) 4 ?
Cs9 O13 3.447(13) . ?
Cs9 O15 3.544(15) . ?
Cs9 O18 2.976(15) . ?
Cs9 O21 3.383(13) 4 ?
Cs9 O33 3.069(16) . ?
Cs10 Zn2 3.711(3) 2_565 ?
Cs10 B5 3.70(2) 2_565 ?
Cs10 B14 3.87(3) 2_565 ?
Cs10 B15 3.54(2) . ?
Cs10 O2 3.060(14) 2_565 ?
Cs10 O10 3.203(14) 2_565 ?
Cs10 O15 3.312(14) 2_565 ?
Cs10 O17 3.065(15) . ?
Cs10 O18 3.130(16) 3_455 ?
Cs10 O30 3.471(16) 2_565 ?
Cs10 O34 3.442(16) . ?
Cs10 O40 3.077(12) 2_565 ?
Cs11 Zn1 3.732(3) . ?
Cs11 B11 3.67(2) . ?
Cs11 B13 3.63(2) 3_445 ?
Cs11 O6 3.457(13) . ?
Cs11 O8 3.087(12) . ?
Cs11 O23 3.191(14) 3_445 ?
Cs11 O24 3.478(18) 3_445 ?
Cs11 O27 3.309(16) 2_565 ?
Cs11 O31 3.263(15) 2 ?
Cs11 O33 3.717(16) 4_455 ?
Cs11 O35 3.786(17) 2 ?
Cs11 O38 3.167(15) . ?
Cs12 B10 3.70(2) 4_455 ?
Cs12 B13 3.59(3) 3_445 ?
Cs12 B17 3.55(2) 4_454 ?
Cs12 B19 3.51(3) . ?
Cs12 O22 2.946(14) 4_454 ?
Cs12 O23 3.232(14) 3_445 ?
Cs12 O24 3.122(17) 3_445 ?
Cs12 O26 3.176(16) 4_455 ?
Cs12 O27 3.512(18) 2_565 ?
Cs12 O29 2.921(16) . ?
Cs12 O39 3.412(14) 4_455 ?
Zn1 O4 1.981(13) 4 ?
Zn1 O22 1.909(15) . ?
Zn1 O31 1.967(14) 2 ?
Zn1 O38 1.934(14) . ?
Zn2 O18 1.927(16) 4_454 ?
Zn2 O24 1.931(14) 3_445 ?
Zn2 O25 1.952(16) . ?
Zn2 O40 1.932(13) . ?
Zn3 O15 1.962(13) . ?
Zn3 O26 1.940(15) . ?
Zn3 O33 1.919(16) . ?
Zn3 O37 1.959(14) 2_564 ?
Zn4 O12 1.949(14) 2_565 ?
Zn4 O16 1.976(14) . ?
Zn4 O17 1.932(15) . ?
Zn4 O29 1.890(16) . ?
B1 O21 1.39(2) 1_556 ?
B1 O38 1.34(2) . ?
B1 O39 1.39(3) 1_556 ?
B2 O11 1.34(3) . ?
B2 O23 1.46(2) . ?
B2 O37 1.34(2) . ?
B3 O13 1.33(3) . ?
B3 O18 1.31(3) . ?
B3 O28 1.44(3) . ?
B4 O6 1.37(3) . ?
B4 O20 1.43(3) . ?
B4 O40 1.31(3) . ?
B5 O2 1.47(3) . ?
B5 O7 1.46(3) . ?
B5 O10 1.47(2) . ?
B5 O21 1.48(2) . ?
B6 O1 1.50(2) . ?
B6 O9 1.45(3) . ?
B6 O11 1.47(2) . ?
B6 O14 1.45(3) . ?
B7 O7 1.38(3) . ?
B7 O31 1.34(3) . ?
B7 O35 1.38(3) . ?
B8 O12 1.38(3) . ?
B8 O14 1.37(3) . ?
B8 O30 1.39(3) . ?
B9 O4 1.35(2) . ?
B9 O19 1.41(3) . ?
B9 O32 1.37(3) . ?
B10 O2 1.36(3) . ?
B10 O26 1.33(3) . ?
B10 O39 1.39(2) . ?
B11 O3 1.47(3) . ?
B11 O6 1.49(3) . ?
B11 O8 1.47(2) . ?
B11 O13 1.48(2) . ?
B12 O5 1.44(3) . ?
B12 O32 1.49(3) . ?
B12 O34 1.44(3) . ?
B12 O36 1.53(3) . ?
B13 O1 1.36(3) . ?
B13 O23 1.45(2) . ?
B13 O24 1.32(3) . ?
B14 O9 1.39(3) . ?
B14 O15 1.32(3) . ?
B14 O30 1.36(3) . ?
B15 O17 1.37(3) . ?
B15 O19 1.37(3) . ?
B15 O34 1.33(3) . ?
B16 O3 1.38(3) . ?
B16 O16 1.33(3) . ?
B16 O20 1.42(3) . ?
B17 O8 1.37(3) . ?
B17 O22 1.32(3) . ?
B17 O28 1.40(3) . ?
B18 O10 1.37(3) . ?
B18 O25 1.35(2) . ?
B18 O35 1.38(3) . ?
B19 O27 1.41(3) 2_565 ?
B19 O29 1.33(3) . ?
B19 O36 1.35(3) 2_565 ?
B20 O5 1.38(3) 3_545 ?
B20 O27 1.39(3) 3_545 ?
B20 O33 1.34(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B1 Cs1 Zn3 112.6(4) 4_554 . ?
B1 Cs1 B2 130.1(5) 4_554 2_564 ?
B1 Cs1 B18 100.0(5) 4_554 3 ?
B2 Cs1 Zn3 47.9(4) 2_564 . ?
B2 Cs1 B18 80.4(5) 2_564 3 ?
B18 Cs1 Zn3 128.3(4) 3 . ?
O1 Cs1 Zn3 98.3(3) . . ?
O1 Cs1 B1 129.4(4) . 4_554 ?
O1 Cs1 B2 100.4(4) . 2_564 ?
O1 Cs1 B18 89.7(4) . 3 ?
O1 Cs1 O9 45.6(3) . . ?
O1 Cs1 O21 111.6(3) . 4 ?
O1 Cs1 O25 69.2(4) . 3 ?
O1 Cs1 O35 111.4(4) . 3 ?
O1 Cs1 O37 89.4(4) . 2_564 ?
O1 Cs1 O38 139.0(4) . 4_554 ?
O9 Cs1 Zn3 57.4(2) . . ?
O9 Cs1 B1 125.0(4) . 4_554 ?
O9 Cs1 B2 85.8(4) . 2_564 ?
O9 Cs1 B18 129.5(4) . 3 ?
O9 Cs1 O21 102.4(3) . 4 ?
O9 Cs1 O35 150.4(4) . 3 ?
O21 Cs1 Zn3 106.2(3) 4 . ?
O21 Cs1 B1 23.2(4) 4 4_554 ?
O21 Cs1 B2 142.3(4) 4 2_564 ?
O21 Cs1 B18 118.0(5) 4 3 ?
O21 Cs1 O35 104.5(4) 4 3 ?
O25 Cs1 Zn3 128.4(3) 3 . ?
O25 Cs1 B1 113.2(5) 3 4_554 ?
O25 Cs1 B2 84.1(5) 3 2_564 ?
O25 Cs1 B18 20.6(4) 3 3 ?
O25 Cs1 O9 110.2(4) 3 . ?
O25 Cs1 O21 125.2(4) 3 4 ?
O25 Cs1 O35 42.5(4) 3 3 ?
O25 Cs1 O37 96.4(4) 3 2_564 ?
O33 Cs1 Zn3 31.3(3) . . ?
O33 Cs1 B1 81.5(5) . 4_554 ?
O33 Cs1 B2 71.3(5) . 2_564 ?
O33 Cs1 B18 142.9(5) . 3 ?
O33 Cs1 O1 118.1(4) . . ?
O33 Cs1 O9 72.5(4) . . ?
O33 Cs1 O21 76.2(4) . 4 ?
O33 Cs1 O25 155.1(4) . 3 ?
O33 Cs1 O35 126.2(4) . 3 ?
O33 Cs1 O37 61.3(4) . 2_564 ?
O33 Cs1 O38 91.2(4) . 4_554 ?
O35 Cs1 Zn3 124.7(3) 3 . ?
O35 Cs1 B1 83.1(4) 3 4_554 ?
O35 Cs1 B2 80.7(5) 3 2_564 ?
O35 Cs1 B18 22.0(4) 3 3 ?
O37 Cs1 Zn3 32.1(3) 2_564 . ?
O37 Cs1 B1 136.9(5) 2_564 4_554 ?
O37 Cs1 B2 20.7(4) 2_564 2_564 ?
O37 Cs1 B18 97.8(5) 2_564 3 ?
O37 Cs1 O9 65.9(3) 2_564 . ?
O37 Cs1 O21 137.5(4) 2_564 4 ?
O37 Cs1 O35 101.0(4) 2_564 3 ?
O38 Cs1 Zn3 119.0(3) 4_554 . ?
O38 Cs1 B1 21.9(4) 4_554 4_554 ?
O38 Cs1 B2 116.7(4) 4_554 2_564 ?
O38 Cs1 B18 80.4(5) 4_554 3 ?
O38 Cs1 O9 146.9(4) 4_554 . ?
O38 Cs1 O21 44.9(3) 4_554 4 ?
O38 Cs1 O25 96.7(4) 4_554 3 ?
O38 Cs1 O35 61.8(4) 4_554 3 ?
O38 Cs1 O37 131.2(4) 4_554 2_564 ?
B8 Cs2 B1 154.7(5) . 2_564 ?
B8 Cs2 B10 125.1(6) . 2_565 ?
B8 Cs2 B11 99.9(5) . 2_564 ?
B8 Cs2 B17 129.9(5) . 2_564 ?
B8 Cs2 O27 93.3(5) . . ?
B10 Cs2 B1 37.7(5) 2_565 2_564 ?
B10 Cs2 B11 131.9(5) 2_565 2_564 ?
B10 Cs2 B17 93.1(6) 2_565 2_564 ?
B11 Cs2 B1 103.7(5) 2_564 2_564 ?
B11 Cs2 B17 39.9(5) 2_564 2_564 ?
B17 Cs2 B1 75.2(5) 2_564 2_564 ?
O3 Cs2 B1 122.4(4) 2_564 2_564 ?
O3 Cs2 B8 78.9(5) 2_564 . ?
O3 Cs2 B10 154.8(5) 2_564 2_565 ?
O3 Cs2 B11 23.0(4) 2_564 2_564 ?
O3 Cs2 B17 62.5(5) 2_564 2_564 ?
O3 Cs2 O8 45.8(4) 2_564 2_564 ?
O3 Cs2 O12 81.3(4) 2_564 . ?
O3 Cs2 O26 155.6(4) 2_564 2_565 ?
O3 Cs2 O27 89.5(3) 2_564 . ?
O3 Cs2 O39 132.9(4) 2_564 2_565 ?
O8 Cs2 B1 82.1(4) 2_564 2_564 ?
O8 Cs2 B8 122.5(4) 2_564 . ?
O8 Cs2 B10 108.9(5) 2_564 2_565 ?
O8 Cs2 B11 23.1(4) 2_564 2_564 ?
O8 Cs2 B17 20.8(4) 2_564 2_564 ?
O8 Cs2 O26 116.7(4) 2_564 2_565 ?
O8 Cs2 O27 99.7(4) 2_564 . ?
O8 Cs2 O39 87.6(4) 2_564 2_565 ?
O12 Cs2 B1 137.6(4) . 2_564 ?
O12 Cs2 B8 23.0(4) . . ?
O12 Cs2 B10 123.7(5) . 2_565 ?
O12 Cs2 B11 104.2(4) . 2_564 ?
O12 Cs2 B17 142.6(5) . 2_564 ?
O12 Cs2 O8 126.9(4) . 2_564 ?
O12 Cs2 O26 115.0(4) . 2_565 ?
O12 Cs2 O27 70.4(4) . . ?
O12 Cs2 O39 142.9(4) . 2_565 ?
O14 Cs2 B1 152.6(4) . 2_564 ?
O14 Cs2 B8 22.5(4) . . ?
O14 Cs2 B10 115.1(5) . 2_565 ?
O14 Cs2 B11 100.0(5) . 2_564 ?
O14 Cs2 B17 117.2(5) . 2_564 ?
O14 Cs2 O3 84.1(4) . 2_564 ?
O14 Cs2 O8 118.5(4) . 2_564 ?
O14 Cs2 O12 45.0(4) . . ?
O14 Cs2 O26 94.9(4) . 2_565 ?
O14 Cs2 O27 115.4(4) . . ?
O14 Cs2 O39 135.0(4) . 2_565 ?
O26 Cs2 B1 58.3(4) 2_565 2_564 ?
O26 Cs2 B8 108.7(5) 2_565 . ?
O26 Cs2 B10 21.4(4) 2_565 2_565 ?
O26 Cs2 B11 136.4(5) 2_565 2_564 ?
O26 Cs2 B17 97.1(5) 2_565 2_564 ?
O26 Cs2 O27 112.6(4) 2_565 . ?
O27 Cs2 B1 74.9(5) . 2_564 ?
O27 Cs2 B10 96.0(5) . 2_565 ?
O27 Cs2 B11 97.5(4) . 2_564 ?
O27 Cs2 B17 115.7(5) . 2_564 ?
O39 Cs2 B1 20.1(4) 2_565 2_564 ?
O39 Cs2 B8 147.6(4) 2_565 . ?
O39 Cs2 B10 22.5(5) 2_565 2_565 ?
O39 Cs2 B11 110.7(4) 2_565 2_564 ?
O39 Cs2 B17 74.4(5) 2_565 2_564 ?
O39 Cs2 O26 40.4(4) 2_565 2_565 ?
O39 Cs2 O27 92.8(4) 2_565 . ?
B7 Cs3 B9 118.8(5) 4_455 . ?
B7 Cs3 B12 97.8(5) 4_455 2_565 ?
B7 Cs3 O39 76.0(4) 4_455 4_455 ?
B9 Cs3 B12 143.4(5) . 2_565 ?
B9 Cs3 O39 88.2(4) . 4_455 ?
B19 Cs3 B7 133.3(6) . 4_455 ?
B19 Cs3 B9 105.2(6) . . ?
B19 Cs3 B12 40.3(6) . 2_565 ?
B19 Cs3 O39 91.2(5) . 4_455 ?
O4 Cs3 B7 99.5(4) . 4_455 ?
O4 Cs3 B9 22.1(4) . . ?
O4 Cs3 B12 159.2(4) . 2_565 ?
O4 Cs3 B19 119.0(5) . . ?
O4 Cs3 O29 97.6(3) . . ?
O4 Cs3 O39 71.8(3) . 4_455 ?
O7 Cs3 B7 22.8(5) 4_455 4_455 ?
O7 Cs3 B9 118.8(5) 4_455 . ?
O7 Cs3 B12 94.7(5) 4_455 2_565 ?
O7 Cs3 B19 119.9(6) 4_455 . ?
O7 Cs3 O4 96.8(4) 4_455 . ?
O7 Cs3 O19 141.0(4) 4_455 . ?
O7 Cs3 O29 133.4(4) 4_455 . ?
O7 Cs3 O31 45.2(4) 4_455 4_455 ?
O7 Cs3 O32 77.2(4) 4_455 2_565 ?
O7 Cs3 O36 116.2(4) 4_455 2_565 ?
O7 Cs3 O39 54.3(3) 4_455 4_455 ?
O19 Cs3 B7 140.0(5) . 4_455 ?
O19 Cs3 B9 22.6(4) . . ?
O19 Cs3 B12 121.5(4) . 2_565 ?
O19 Cs3 B19 86.1(5) . . ?
O19 Cs3 O4 44.3(3) . . ?
O19 Cs3 O29 64.9(4) . . ?
O19 Cs3 O31 126.7(4) . 4_455 ?
O19 Cs3 O32 141.4(4) . 2_565 ?
O19 Cs3 O36 98.7(4) . 2_565 ?
O19 Cs3 O39 100.8(4) . 4_455 ?
O29 Cs3 B7 152.6(5) . 4_455 ?
O29 Cs3 B9 83.1(5) . . ?
O29 Cs3 B12 62.1(4) . 2_565 ?
O29 Cs3 B19 22.1(5) . . ?
O29 Cs3 O39 89.3(3) . 4_455 ?
O31 Cs3 B7 22.6(5) 4_455 4_455 ?
O31 Cs3 B9 110.4(5) 4_455 . ?
O31 Cs3 B12 103.5(4) 4_455 2_565 ?
O31 Cs3 B19 143.8(5) 4_455 . ?
O31 Cs3 O4 96.9(3) 4_455 . ?
O31 Cs3 O29 165.4(4) 4_455 . ?
O31 Cs3 O39 96.3(4) 4_455 4_455 ?
O32 Cs3 B7 76.0(4) 2_565 4_455 ?
O32 Cs3 B9 164.0(4) 2_565 . ?
O32 Cs3 B12 22.7(4) 2_565 2_565 ?
O32 Cs3 B19 62.9(5) 2_565 . ?
O32 Cs3 O4 173.4(3) 2_565 . ?
O32 Cs3 O29 84.8(3) 2_565 . ?
O32 Cs3 O31 80.9(3) 2_565 4_455 ?
O32 Cs3 O39 102.1(3) 2_565 4_455 ?
O36 Cs3 B7 120.5(5) 2_565 4_455 ?
O36 Cs3 B9 120.7(5) 2_565 . ?
O36 Cs3 B12 22.8(4) 2_565 2_565 ?
O36 Cs3 B19 22.7(5) 2_565 . ?
O36 Cs3 O4 138.8(3) 2_565 . ?
O36 Cs3 O29 41.9(4) 2_565 . ?
O36 Cs3 O31 123.6(4) 2_565 4_455 ?
O36 Cs3 O32 44.7(3) 2_565 2_565 ?
O36 Cs3 O39 107.1(4) 2_565 4_455 ?
O39 Cs3 B12 101.5(5) 4_455 2_565 ?
Zn4 Cs4 Cs10 71.63(8) 2_564 2_564 ?
B12 Cs4 Cs10 146.6(3) . 2_564 ?
B12 Cs4 Zn4 75.7(3) . 2_564 ?
B15 Cs4 Cs10 166.9(4) . 2_564 ?
B15 Cs4 Zn4 106.3(4) . 2_564 ?
B15 Cs4 B12 36.7(5) . . ?
B15 Cs4 O34 20.2(4) . . ?
B16 Cs4 Cs10 87.3(3) . 2_564 ?
B16 Cs4 Zn4 122.0(4) . 2_564 ?
B16 Cs4 B12 116.5(5) . . ?
B16 Cs4 B15 83.0(5) . . ?
B16 Cs4 O34 95.1(4) . . ?
O12 Cs4 Cs10 82.7(3) . 2_564 ?
O12 Cs4 Zn4 29.8(2) . 2_564 ?
O12 Cs4 B12 72.1(4) . . ?
O12 Cs4 B15 89.6(4) . . ?
O12 Cs4 B16 96.3(4) . . ?
O12 Cs4 O17 55.1(3) . 2_564 ?
O12 Cs4 O34 72.2(3) . . ?
O16 Cs4 Cs10 105.5(3) . 2_564 ?
O16 Cs4 Zn4 118.1(3) . 2_564 ?
O16 Cs4 B12 95.7(4) . . ?
O16 Cs4 B15 63.5(4) . . ?
O16 Cs4 B16 20.8(4) . . ?
O16 Cs4 O12 88.7(3) . . ?
O16 Cs4 O17 133.1(3) . 2_564 ?
O16 Cs4 O28 124.8(5) . 4_454 ?
O16 Cs4 O34 74.3(3) . . ?
O17 Cs4 Cs10 47.5(3) 2_564 2_564 ?
O17 Cs4 Zn4 29.4(2) 2_564 2_564 ?
O17 Cs4 B12 99.3(4) 2_564 . ?
O17 Cs4 B15 134.0(4) 2_564 . ?
O17 Cs4 B16 124.9(4) 2_564 . ?
O17 Cs4 O34 114.0(3) 2_564 . ?
O20 Cs4 Cs10 69.8(3) . 2_564 ?
O20 Cs4 Zn4 123.8(3) . 2_564 ?
O20 Cs4 B12 137.7(5) . . ?
O20 Cs4 B15 102.5(5) . . ?
O20 Cs4 B16 21.7(5) . . ?
O20 Cs4 O12 105.9(4) . . ?
O20 Cs4 O16 42.5(4) . . ?
O20 Cs4 O17 114.2(4) . 2_564 ?
O20 Cs4 O28 91.6(5) . 4_454 ?
O20 Cs4 O34 116.4(4) . . ?
O20 Cs4 O36 150.3(4) . . ?
O28 Cs4 Cs10 71.7(3) 4_454 2_564 ?
O28 Cs4 Zn4 113.0(3) 4_454 2_564 ?
O28 Cs4 B12 116.3(5) 4_454 . ?
O28 Cs4 B15 120.0(5) 4_454 . ?
O28 Cs4 B16 109.9(6) 4_454 . ?
O28 Cs4 O12 141.8(4) 4_454 . ?
O28 Cs4 O17 86.8(4) 4_454 2_564 ?
O28 Cs4 O34 129.7(4) 4_454 . ?
O34 Cs4 Cs10 154.9(2) . 2_564 ?
O34 Cs4 Zn4 86.2(2) . 2_564 ?
O34 Cs4 B12 21.4(4) . . ?
O36 Cs4 Cs10 124.6(3) . 2_564 ?
O36 Cs4 Zn4 54.3(3) . 2_564 ?
O36 Cs4 B12 22.0(4) . . ?
O36 Cs4 B15 57.5(4) . . ?
O36 Cs4 B16 129.1(5) . . ?
O36 Cs4 O12 56.7(4) . . ?
O36 Cs4 O16 109.0(4) . . ?
O36 Cs4 O17 77.5(4) . 2_564 ?
O36 Cs4 O28 117.1(4) . 4_454 ?
O36 Cs4 O34 39.0(3) . . ?
B2 Cs5 B3 136.2(5) 2_564 2_564 ?
B2 Cs5 B6 101.3(5) 2_564 . ?
B2 Cs5 O16 100.6(4) 2_564 2_564 ?
B6 Cs5 B3 113.2(5) . 2_564 ?
B16 Cs5 B2 115.3(5) 2_564 2_564 ?
B16 Cs5 B3 80.6(6) 2_564 2_564 ?
B16 Cs5 B6 106.4(5) 2_564 . ?
B16 Cs5 O16 21.8(4) 2_564 2_564 ?
O1 Cs5 B2 106.0(4) . 2_564 ?
O1 Cs5 B3 96.4(5) . 2_564 ?
O1 Cs5 B6 24.1(4) . . ?
O1 Cs5 B16 122.4(4) . 2_564 ?
O1 Cs5 O3 108.5(4) . 2_564 ?
O1 Cs5 O11 126.2(4) . 2_564 ?
O1 Cs5 O13 113.4(4) . 2_564 ?
O1 Cs5 O14 42.8(3) . . ?
O1 Cs5 O16 116.5(3) . 2_564 ?
O1 Cs5 O25 67.0(4) . 3 ?
O1 Cs5 O37 88.7(3) . 2_564 ?
O3 Cs5 B2 138.0(4) 2_564 2_564 ?
O3 Cs5 B3 61.8(5) 2_564 2_564 ?
O3 Cs5 B6 100.5(4) 2_564 . ?
O3 Cs5 B16 23.2(5) 2_564 2_564 ?
O3 Cs5 O13 45.5(3) 2_564 2_564 ?
O3 Cs5 O14 77.6(3) 2_564 . ?
O3 Cs5 O16 41.9(4) 2_564 2_564 ?
O3 Cs5 O25 131.7(4) 2_564 3 ?
O3 Cs5 O37 138.1(3) 2_564 2_564 ?
O11 Cs5 B2 22.4(4) 2_564 2_564 ?
O11 Cs5 B3 117.5(5) 2_564 2_564 ?
O11 Cs5 B6 123.7(4) 2_564 . ?
O11 Cs5 B16 104.3(5) 2_564 2_564 ?
O11 Cs5 O3 123.8(4) 2_564 2_564 ?
O11 Cs5 O13 111.7(4) 2_564 2_564 ?
O11 Cs5 O14 135.3(4) 2_564 . ?
O11 Cs5 O16 96.7(4) 2_564 2_564 ?
O11 Cs5 O25 85.3(4) 2_564 3 ?
O11 Cs5 O37 44.4(3) 2_564 2_564 ?
O13 Cs5 B2 133.9(4) 2_564 2_564 ?
O13 Cs5 B3 21.5(5) 2_564 2_564 ?
O13 Cs5 B6 124.4(4) 2_564 . ?
O13 Cs5 B16 60.8(5) 2_564 2_564 ?
O13 Cs5 O14 110.1(3) 2_564 . ?
O13 Cs5 O16 82.6(4) 2_564 2_564 ?
O13 Cs5 O25 90.3(4) 2_564 3 ?
O13 Cs5 O37 156.0(3) 2_564 2_564 ?
O14 Cs5 B2 115.0(4) . 2_564 ?
O14 Cs5 B3 107.1(4) . 2_564 ?
O14 Cs5 B6 23.8(4) . . ?
O14 Cs5 B16 82.8(4) . 2_564 ?
O14 Cs5 O16 73.6(3) . 2_564 ?
O16 Cs5 B3 102.2(5) 2_564 2_564 ?
O16 Cs5 B6 95.0(4) 2_564 . ?
O25 Cs5 B2 83.8(4) 3 2_564 ?
O25 Cs5 B3 70.8(5) 3 2_564 ?
O25 Cs5 B6 89.5(5) 3 . ?
O25 Cs5 B16 151.1(5) 3 2_564 ?
O25 Cs5 O14 109.7(3) 3 . ?
O25 Cs5 O16 172.9(4) 3 2_564 ?
O37 Cs5 B2 22.6(4) 2_564 2_564 ?
O37 Cs5 B3 156.2(5) 2_564 2_564 ?
O37 Cs5 B6 79.7(4) 2_564 . ?
O37 Cs5 B16 116.1(5) 2_564 2_564 ?
O37 Cs5 O14 92.4(3) 2_564 . ?
O37 Cs5 O16 96.1(3) 2_564 2_564 ?
O37 Cs5 O25 90.1(4) 2_564 3 ?
B4 Cs6 Zn2 47.2(4) 3_455 3_455 ?
B4 Cs6 O7 139.5(4) 3_455 4_455 ?
B7 Cs6 Zn2 128.3(4) 4_455 3_455 ?
B7 Cs6 B4 118.1(5) 4_455 3_455 ?
B7 Cs6 B18 150.1(6) 4_455 3_455 ?
B7 Cs6 O7 22.1(4) 4_455 4_455 ?
B7 Cs6 O35 137.9(5) 4_455 3_455 ?
B18 Cs6 Zn2 45.8(4) 3_455 3_455 ?
B18 Cs6 B4 79.9(6) 3_455 3_455 ?
B18 Cs6 O7 137.8(5) 3_455 4_455 ?
O4 Cs6 Zn2 124.2(3) . 3_455 ?
O4 Cs6 B4 113.9(4) . 3_455 ?
O4 Cs6 B7 107.1(5) . 4_455 ?
O4 Cs6 B18 83.8(4) . 3_455 ?
O4 Cs6 O6 106.5(4) . 3_455 ?
O4 Cs6 O7 89.2(3) . 4_455 ?
O4 Cs6 O25 105.4(3) . 3_455 ?
O4 Cs6 O31 105.9(4) . 4_455 ?
O4 Cs6 O35 68.1(3) . 3_455 ?
O4 Cs6 O38 59.3(3) . 4_454 ?
O4 Cs6 O40 110.2(3) . 3_455 ?
O6 Cs6 Zn2 68.7(2) 3_455 3_455 ?
O6 Cs6 B4 21.7(4) 3_455 3_455 ?
O6 Cs6 B7 103.8(5) 3_455 4_455 ?
O6 Cs6 B18 99.3(5) 3_455 3_455 ?
O6 Cs6 O7 122.5(3) 3_455 4_455 ?
O6 Cs6 O25 97.0(4) 3_455 3_455 ?
O6 Cs6 O31 82.7(4) 3_455 4_455 ?
O6 Cs6 O35 117.8(3) 3_455 3_455 ?
O6 Cs6 O38 165.3(3) 3_455 4_454 ?
O6 Cs6 O40 42.2(3) 3_455 3_455 ?
O7 Cs6 Zn2 142.1(2) 4_455 3_455 ?
O25 Cs6 Zn2 30.9(3) 3_455 3_455 ?
O25 Cs6 B4 75.4(5) 3_455 3_455 ?
O25 Cs6 B7 134.0(4) 3_455 4_455 ?
O25 Cs6 B18 22.0(4) 3_455 3_455 ?
O25 Cs6 O7 132.1(3) 3_455 4_455 ?
O25 Cs6 O35 39.0(3) 3_455 3_455 ?
O25 Cs6 O38 84.4(4) 3_455 4_454 ?
O25 Cs6 O40 55.1(4) 3_455 3_455 ?
O31 Cs6 Zn2 127.1(3) 4_455 3_455 ?
O31 Cs6 B4 99.9(5) 4_455 3_455 ?
O31 Cs6 B7 22.7(5) 4_455 4_455 ?
O31 Cs6 B18 169.2(5) 4_455 3_455 ?
O31 Cs6 O7 40.1(4) 4_455 4_455 ?
O31 Cs6 O25 147.4(3) 4_455 3_455 ?
O31 Cs6 O35 159.4(4) 4_455 3_455 ?
O31 Cs6 O38 103.9(4) 4_455 4_454 ?
O31 Cs6 O40 120.1(4) 4_455 3_455 ?
O35 Cs6 Zn2 67.2(2) 3_455 3_455 ?
O35 Cs6 B4 100.5(4) 3_455 3_455 ?
O35 Cs6 B18 22.1(4) 3_455 3_455 ?
O35 Cs6 O7 119.3(3) 3_455 4_455 ?
O38 Cs6 Zn2 115.0(2) 4_454 3_455 ?
O38 Cs6 B4 156.2(4) 4_454 3_455 ?
O38 Cs6 B7 85.1(5) 4_454 4_455 ?
O38 Cs6 B18 76.7(5) 4_454 3_455 ?
O38 Cs6 O7 64.2(3) 4_454 4_455 ?
O38 Cs6 O35 55.7(3) 4_454 3_455 ?
O40 Cs6 Zn2 30.5(2) 3_455 3_455 ?
O40 Cs6 B4 21.2(4) 3_455 3_455 ?
O40 Cs6 B7 135.3(5) 3_455 4_455 ?
O40 Cs6 B18 58.8(5) 3_455 3_455 ?
O40 Cs6 O7 157.4(3) 3_455 4_455 ?
O40 Cs6 O35 79.9(3) 3_455 3_455 ?
O40 Cs6 O38 135.5(3) 3_455 4_454 ?
B4 Cs7 B5 103.1(5) 3_455 3_455 ?
B4 Cs7 B9 118.3(6) 3_455 . ?
B4 Cs7 B12 148.1(5) 3_455 . ?
B4 Cs7 O4 103.1(5) 3_455 . ?
B4 Cs7 O7 115.0(5) 3_455 3_455 ?
B5 Cs7 O7 22.6(4) 3_455 3_455 ?
B9 Cs7 B5 95.3(5) . 3_455 ?
B9 Cs7 B12 41.3(5) . . ?
B9 Cs7 O4 21.6(4) . . ?
B9 Cs7 O7 72.7(4) . 3_455 ?
B12 Cs7 B5 103.3(5) . 3_455 ?
B12 Cs7 O4 62.3(4) . . ?
B12 Cs7 O7 85.0(5) . 3_455 ?
O2 Cs7 B4 110.0(5) 3_455 3_455 ?
O2 Cs7 B5 22.5(5) 3_455 3_455 ?
O2 Cs7 B9 108.7(4) 3_455 . ?
O2 Cs7 B12 101.2(5) 3_455 . ?
O2 Cs7 O4 103.0(4) 3_455 . ?
O2 Cs7 O5 99.5(4) 3_455 . ?
O2 Cs7 O6 131.5(3) 3_455 3_455 ?
O2 Cs7 O7 39.7(4) 3_455 3_455 ?
O2 Cs7 O15 73.2(4) 3_455 3_455 ?
O2 Cs7 O40 89.7(3) 3_455 3_455 ?
O4 Cs7 B5 84.2(5) . 3_455 ?
O4 Cs7 O7 63.4(3) . 3_455 ?
O5 Cs7 B4 146.3(5) . 3_455 ?
O5 Cs7 B5 110.3(4) . 3_455 ?
O5 Cs7 B9 63.7(4) . . ?
O5 Cs7 B12 22.9(5) . . ?
O5 Cs7 O4 85.0(3) . . ?
O5 Cs7 O6 128.6(3) . 3_455 ?
O5 Cs7 O7 98.1(4) . 3_455 ?
O5 Cs7 O40 168.4(4) . 3_455 ?
O6 Cs7 B4 23.3(5) 3_455 3_455 ?
O6 Cs7 B5 119.5(4) 3_455 3_455 ?
O6 Cs7 B9 98.5(4) 3_455 . ?
O6 Cs7 B12 124.9(4) 3_455 . ?
O6 Cs7 O4 87.9(3) 3_455 . ?
O6 Cs7 O7 123.4(3) 3_455 3_455 ?
O15 Cs7 B4 90.8(5) 3_455 3_455 ?
O15 Cs7 B5 94.4(5) 3_455 3_455 ?
O15 Cs7 B9 146.0(4) 3_455 . ?
O15 Cs7 B12 104.8(5) 3_455 . ?
O15 Cs7 O4 166.0(3) 3_455 . ?
O15 Cs7 O5 82.4(4) 3_455 . ?
O15 Cs7 O6 104.8(3) 3_455 3_455 ?
O15 Cs7 O7 112.3(3) 3_455 3_455 ?
O15 Cs7 O40 93.7(4) 3_455 3_455 ?
O32 Cs7 B4 140.6(5) . 3_455 ?
O32 Cs7 B5 89.7(5) . 3_455 ?
O32 Cs7 B9 22.3(4) . . ?
O32 Cs7 B12 23.5(5) . . ?
O32 Cs7 O2 96.0(4) . 3_455 ?
O32 Cs7 O4 40.6(3) . . ?
O32 Cs7 O5 46.2(4) . . ?
O32 Cs7 O6 119.7(3) . 3_455 ?
O32 Cs7 O7 68.2(3) . 3_455 ?
O32 Cs7 O15 125.6(4) . 3_455 ?
O32 Cs7 O40 140.3(4) . 3_455 ?
O40 Cs7 B4 22.4(4) 3_455 3_455 ?
O40 Cs7 B5 80.8(4) 3_455 3_455 ?
O40 Cs7 B9 120.0(4) 3_455 . ?
O40 Cs7 B12 160.6(5) 3_455 . ?
O40 Cs7 O4 99.9(3) 3_455 . ?
O40 Cs7 O6 41.9(3) 3_455 3_455 ?
O40 Cs7 O7 93.5(3) 3_455 3_455 ?
Zn4 Cs8 O11 120.0(2) . . ?
B2 Cs8 Zn4 128.7(3) . . ?
B2 Cs8 O11 21.1(4) . . ?
B8 Cs8 Zn4 122.5(5) . . ?
B8 Cs8 B2 68.9(5) . . ?
B8 Cs8 B15 116.2(5) . . ?
B8 Cs8 O11 54.3(4) . . ?
B15 Cs8 Zn4 47.9(4) . . ?
B15 Cs8 B2 174.7(5) . . ?
B15 Cs8 O11 161.1(5) . . ?
O12 Cs8 Zn4 119.6(3) . . ?
O12 Cs8 B2 88.5(4) . . ?
O12 Cs8 B8 23.0(4) . . ?
O12 Cs8 B15 96.8(4) . . ?
O12 Cs8 O11 76.6(3) . . ?
O12 Cs8 O14 40.5(3) . . ?
O12 Cs8 O30 170.7(4) . 2_565 ?
O14 Cs8 Zn4 138.8(3) . . ?
O14 Cs8 B2 48.0(4) . . ?
O14 Cs8 B8 22.4(4) . . ?
O14 Cs8 B15 137.3(4) . . ?
O14 Cs8 O11 38.0(3) . . ?
O14 Cs8 O30 140.3(4) . 2_565 ?
O16 Cs8 Zn4 32.3(3) . . ?
O16 Cs8 B2 109.2(5) . . ?
O16 Cs8 B8 92.9(5) . . ?
O16 Cs8 B15 69.8(5) . . ?
O16 Cs8 O11 93.3(4) . . ?
O16 Cs8 O12 97.9(4) . . ?
O16 Cs8 O14 106.6(4) . . ?
O16 Cs8 O17 61.4(4) . . ?
O16 Cs8 O30 72.9(4) . 2_565 ?
O16 Cs8 O34 88.5(4) . . ?
O16 Cs8 O37 107.4(4) . . ?
O17 Cs8 Zn4 31.6(3) . . ?
O17 Cs8 B2 152.1(4) . . ?
O17 Cs8 B8 134.3(5) . . ?
O17 Cs8 B15 22.8(4) . . ?
O17 Cs8 O11 151.1(3) . . ?
O17 Cs8 O12 118.0(3) . . ?
O17 Cs8 O14 156.7(3) . . ?
O17 Cs8 O30 58.7(3) . 2_565 ?
O17 Cs8 O34 43.1(4) . . ?
O30 Cs8 Zn4 52.6(3) 2_565 . ?
O30 Cs8 B2 93.7(4) 2_565 . ?
O30 Cs8 B8 152.9(5) 2_565 . ?
O30 Cs8 B15 81.0(4) 2_565 . ?
O30 Cs8 O11 102.6(3) 2_565 . ?
O34 Cs8 Zn4 69.8(3) . . ?
O34 Cs8 B2 161.2(5) . . ?
O34 Cs8 B8 105.2(5) . . ?
O34 Cs8 B15 22.0(4) . . ?
O34 Cs8 O11 159.5(3) . . ?
O34 Cs8 O12 82.9(4) . . ?
O34 Cs8 O14 122.2(3) . . ?
O34 Cs8 O30 97.5(4) . 2_565 ?
O37 Cs8 Zn4 115.6(2) . . ?
O37 Cs8 B2 21.8(4) . . ?
O37 Cs8 B8 90.6(4) . . ?
O37 Cs8 B15 152.9(4) . . ?
O37 Cs8 O11 39.1(3) . . ?
O37 Cs8 O12 110.2(3) . . ?
O37 Cs8 O14 69.8(3) . . ?
O37 Cs8 O17 131.4(3) . . ?
O37 Cs8 O30 72.7(3) . 2_565 ?
O37 Cs8 O34 157.2(4) . . ?
B3 Cs9 B14 113.4(6) . . ?
B3 Cs9 B18 83.0(6) . 4 ?
B3 Cs9 O15 110.2(5) . . ?
B18 Cs9 B14 127.2(6) 4 . ?
B20 Cs9 B3 119.3(6) . . ?
B20 Cs9 B14 85.7(6) . . ?
B20 Cs9 B18 131.1(6) . 4 ?
B20 Cs9 O15 68.5(5) . . ?
O5 Cs9 B3 95.9(5) 3_545 . ?
O5 Cs9 B14 94.4(5) 3_545 . ?
O5 Cs9 B18 135.2(5) 3_545 4 ?
O5 Cs9 B20 23.5(5) 3_545 . ?
O5 Cs9 O13 97.4(4) 3_545 . ?
O5 Cs9 O15 73.8(3) 3_545 . ?
O5 Cs9 O21 90.1(3) 3_545 4 ?
O9 Cs9 B3 124.4(5) . . ?
O9 Cs9 B14 22.0(5) . . ?
O9 Cs9 B18 107.0(5) . 4 ?
O9 Cs9 B20 95.0(5) . . ?
O9 Cs9 O5 110.0(4) . 3_545 ?
O9 Cs9 O13 104.0(3) . . ?
O9 Cs9 O15 41.5(3) . . ?
O9 Cs9 O21 100.6(3) . 4 ?
O9 Cs9 O33 73.5(4) . . ?
O10 Cs9 B3 87.6(5) 4 . ?
O10 Cs9 B14 143.4(5) 4 . ?
O10 Cs9 B18 21.9(5) 4 4 ?
O10 Cs9 B20 110.5(5) 4 . ?
O10 Cs9 O5 113.6(4) 4 3_545 ?
O10 Cs9 O9 121.5(4) 4 . ?
O10 Cs9 O13 106.9(3) 4 . ?
O10 Cs9 O15 160.4(3) 4 . ?
O10 Cs9 O21 44.3(3) 4 4 ?
O10 Cs9 O33 115.9(4) 4 . ?
O13 Cs9 B3 22.0(5) . . ?
O13 Cs9 B14 91.4(5) . . ?
O13 Cs9 B18 97.2(4) . 4 ?
O13 Cs9 B20 119.4(5) . . ?
O13 Cs9 O15 89.5(3) . . ?
O15 Cs9 B14 21.2(5) . . ?
O15 Cs9 B18 148.3(5) . 4 ?
O18 Cs9 B3 21.2(5) . . ?
O18 Cs9 B14 131.8(5) . . ?
O18 Cs9 B18 64.1(5) . 4 ?
O18 Cs9 B20 123.7(6) . . ?
O18 Cs9 O5 102.4(4) . 3_545 ?
O18 Cs9 O9 136.4(4) . . ?
O18 Cs9 O10 66.6(4) . 4 ?
O18 Cs9 O13 42.1(4) . . ?
O18 Cs9 O15 131.3(4) . . ?
O18 Cs9 O21 107.8(3) . 4 ?
O18 Cs9 O33 146.3(5) . . ?
O21 Cs9 B3 128.4(5) 4 . ?
O21 Cs9 B14 117.1(5) 4 . ?
O21 Cs9 B18 58.8(4) 4 4 ?
O21 Cs9 B20 74.8(5) 4 . ?
O21 Cs9 O13 149.9(3) 4 . ?
O21 Cs9 O15 120.5(3) 4 . ?
O33 Cs9 B3 138.6(5) . . ?
O33 Cs9 B14 68.2(5) . . ?
O33 Cs9 B18 131.0(5) . 4 ?
O33 Cs9 B20 22.7(5) . . ?
O33 Cs9 O5 44.4(4) . 3_545 ?
O33 Cs9 O13 131.0(4) . . ?
O33 Cs9 O15 55.6(4) . . ?
O33 Cs9 O21 72.8(4) . 4 ?
Zn2 Cs10 B14 125.5(4) 2_565 2_565 ?
B5 Cs10 Zn2 77.6(4) 2_565 2_565 ?
B5 Cs10 B14 109.7(5) 2_565 2_565 ?
B15 Cs10 Zn2 120.3(4) . 2_565 ?
B15 Cs10 B5 126.8(5) . 2_565 ?
B15 Cs10 B14 98.5(6) . 2_565 ?
O2 Cs10 Zn2 95.9(3) 2_565 2_565 ?
O2 Cs10 B5 22.8(4) 2_565 2_565 ?
O2 Cs10 B14 88.0(5) 2_565 2_565 ?
O2 Cs10 B15 126.9(5) 2_565 . ?
O2 Cs10 O10 44.9(3) 2_565 2_565 ?
O2 Cs10 O15 69.2(3) 2_565 2_565 ?
O2 Cs10 O17 136.0(4) 2_565 . ?
O2 Cs10 O18 107.3(4) 2_565 3_455 ?
O2 Cs10 O30 107.4(4) 2_565 2_565 ?
O2 Cs10 O34 105.8(4) 2_565 . ?
O2 Cs10 O40 90.7(4) 2_565 2_565 ?
O10 Cs10 Zn2 55.2(2) 2_565 2_565 ?
O10 Cs10 B5 23.2(4) 2_565 2_565 ?
O10 Cs10 B14 125.5(5) 2_565 2_565 ?
O10 Cs10 B15 129.4(4) 2_565 . ?
O10 Cs10 O15 107.0(3) 2_565 2_565 ?
O10 Cs10 O30 145.7(4) 2_565 2_565 ?
O10 Cs10 O34 111.8(4) 2_565 . ?
O15 Cs10 Zn2 121.9(3) 2_565 2_565 ?
O15 Cs10 B5 90.5(4) 2_565 2_565 ?
O15 Cs10 B14 19.2(5) 2_565 2_565 ?
O15 Cs10 B15 112.2(5) 2_565 . ?
O15 Cs10 O30 39.5(4) 2_565 2_565 ?
O15 Cs10 O34 113.2(4) 2_565 . ?
O17 Cs10 Zn2 126.0(3) . 2_565 ?
O17 Cs10 B5 145.3(4) . 2_565 ?
O17 Cs10 B14 78.7(5) . 2_565 ?
O17 Cs10 B15 22.5(4) . . ?
O17 Cs10 O10 151.9(3) . 2_565 ?
O17 Cs10 O15 95.1(3) . 2_565 ?
O17 Cs10 O18 103.9(4) . 3_455 ?
O17 Cs10 O30 60.2(4) . 2_565 ?
O17 Cs10 O34 41.5(4) . . ?
O17 Cs10 O40 131.7(4) . 2_565 ?
O18 Cs10 Zn2 31.3(3) 3_455 2_565 ?
O18 Cs10 B5 84.7(5) 3_455 2_565 ?
O18 Cs10 B14 151.2(4) 3_455 2_565 ?
O18 Cs10 B15 91.5(5) 3_455 . ?
O18 Cs10 O10 62.7(4) 3_455 2_565 ?
O18 Cs10 O15 153.1(4) 3_455 2_565 ?
O18 Cs10 O30 140.9(4) 3_455 2_565 ?
O18 Cs10 O34 93.6(4) 3_455 . ?
O30 Cs10 Zn2 127.3(3) 2_565 2_565 ?
O30 Cs10 B5 129.7(4) 2_565 2_565 ?
O30 Cs10 B14 20.5(5) 2_565 2_565 ?
O30 Cs10 B15 81.6(5) 2_565 . ?
O34 Cs10 Zn2 124.8(3) . 2_565 ?
O34 Cs10 B5 105.3(4) . 2_565 ?
O34 Cs10 B14 105.7(5) . 2_565 ?
O34 Cs10 B15 21.8(4) . . ?
O34 Cs10 O30 93.7(4) . 2_565 ?
O40 Cs10 Zn2 31.3(2) 2_565 2_565 ?
O40 Cs10 B5 82.2(5) 2_565 2_565 ?
O40 Cs10 B14 94.5(4) 2_565 2_565 ?
O40 Cs10 B15 140.3(5) 2_565 . ?
O40 Cs10 O10 66.4(3) 2_565 2_565 ?
O40 Cs10 O15 91.2(3) 2_565 2_565 ?
O40 Cs10 O18 61.9(4) 2_565 3_455 ?
O40 Cs10 O30 100.4(4) 2_565 2_565 ?
O40 Cs10 O34 154.0(4) 2_565 . ?
Zn1 Cs11 O35 49.5(3) . 2 ?
B11 Cs11 Zn1 79.0(3) . . ?
B11 Cs11 O33 140.5(4) . 4_455 ?
B11 Cs11 O35 114.2(4) . 2 ?
B13 Cs11 Zn1 130.8(5) 3_445 . ?
B13 Cs11 B11 113.2(5) 3_445 . ?
B13 Cs11 O33 91.3(4) 3_445 4_455 ?
B13 Cs11 O35 84.4(5) 3_445 2 ?
O6 Cs11 Zn1 90.4(2) . . ?
O6 Cs11 B11 23.8(4) . . ?
O6 Cs11 B13 89.9(4) . 3_445 ?
O6 Cs11 O24 71.3(3) . 3_445 ?
O6 Cs11 O33 153.2(3) . 4_455 ?
O6 Cs11 O35 108.8(3) . 2 ?
O8 Cs11 Zn1 56.7(3) . . ?
O8 Cs11 B11 23.0(4) . . ?
O8 Cs11 B13 130.6(4) . 3_445 ?
O8 Cs11 O6 42.3(3) . . ?
O8 Cs11 O23 153.8(3) . 3_445 ?
O8 Cs11 O24 113.6(3) . 3_445 ?
O8 Cs11 O27 107.1(4) . 2_565 ?
O8 Cs11 O31 60.8(4) . 2 ?
O8 Cs11 O33 136.2(3) . 4_455 ?
O8 Cs11 O35 98.2(3) . 2 ?
O8 Cs11 O38 78.8(3) . . ?
O23 Cs11 Zn1 133.6(3) 3_445 . ?
O23 Cs11 B11 134.2(4) 3_445 . ?
O23 Cs11 B13 23.4(4) 3_445 3_445 ?
O23 Cs11 O6 112.1(3) 3_445 . ?
O23 Cs11 O24 40.9(3) 3_445 3_445 ?
O23 Cs11 O27 88.7(4) 3_445 2_565 ?
O23 Cs11 O31 114.0(4) 3_445 2 ?
O23 Cs11 O33 68.3(3) 3_445 4_455 ?
O23 Cs11 O35 84.4(4) 3_445 2 ?
O24 Cs11 Zn1 137.8(3) 3_445 . ?
O24 Cs11 B11 93.5(4) 3_445 . ?
O24 Cs11 B13 21.2(5) 3_445 3_445 ?
O24 Cs11 O33 103.2(4) 3_445 4_455 ?
O24 Cs11 O35 99.9(4) 3_445 2 ?
O27 Cs11 Zn1 118.2(3) 2_565 . ?
O27 Cs11 B11 103.0(5) 2_565 . ?
O27 Cs11 B13 105.5(5) 2_565 3_445 ?
O27 Cs11 O6 115.9(4) 2_565 . ?
O27 Cs11 O24 104.0(4) 2_565 3_445 ?
O27 Cs11 O33 38.5(4) 2_565 4_455 ?
O27 Cs11 O35 134.0(4) 2_565 2 ?
O31 Cs11 Zn1 31.8(2) 2 . ?
O31 Cs11 B11 75.9(5) 2 . ?
O31 Cs11 B13 102.2(5) 2 3_445 ?
O31 Cs11 O6 75.1(3) 2 . ?
O31 Cs11 O24 106.0(4) 2 3_445 ?
O31 Cs11 O27 150.0(4) 2 2_565 ?
O31 Cs11 O33 130.6(3) 2 4_455 ?
O31 Cs11 O35 38.4(3) 2 2 ?
O33 Cs11 Zn1 108.7(2) 4_455 . ?
O33 Cs11 O35 98.0(3) 4_455 2 ?
O38 Cs11 Zn1 31.2(2) . . ?
O38 Cs11 B11 101.6(4) . . ?
O38 Cs11 B13 135.4(5) . 3_445 ?
O38 Cs11 O6 118.8(3) . . ?
O38 Cs11 O23 122.3(3) . 3_445 ?
O38 Cs11 O24 154.8(4) . 3_445 ?
O38 Cs11 O27 92.2(4) . 2_565 ?
O38 Cs11 O31 59.4(4) . 2 ?
O38 Cs11 O33 77.6(3) . 4_455 ?
O38 Cs11 O35 55.5(4) . 2 ?
B10 Cs12 Cs11 114.6(4) 4_455 . ?
B13 Cs12 Cs11 56.4(4) 3_445 . ?
B13 Cs12 B10 103.0(6) 3_445 4_455 ?
B17 Cs12 Cs11 138.7(4) 4_454 . ?
B17 Cs12 B10 94.5(5) 4_454 4_455 ?
B17 Cs12 B13 90.1(6) 4_454 3_445 ?
B19 Cs12 Cs11 70.2(5) . . ?
B19 Cs12 B10 85.4(6) . 4_455 ?
B19 Cs12 B13 124.6(6) . 3_445 ?
B19 Cs12 B17 144.5(6) . 4_454 ?
B19 Cs12 O27 23.1(5) . 2_565 ?
O22 Cs12 Cs11 156.3(3) 4_454 . ?
O22 Cs12 B10 86.7(5) 4_454 4_455 ?
O22 Cs12 B13 110.7(5) 4_454 3_445 ?
O22 Cs12 B17 20.9(5) 4_454 4_454 ?
O22 Cs12 B19 124.5(6) 4_454 . ?
O22 Cs12 O23 126.3(4) 4_454 3_445 ?
O22 Cs12 O24 104.1(5) 4_454 3_445 ?
O22 Cs12 O26 104.0(4) 4_454 4_455 ?
O22 Cs12 O27 147.0(4) 4_454 2_565 ?
O22 Cs12 O39 64.6(4) 4_454 4_455 ?
O23 Cs12 Cs11 50.4(2) 3_445 . ?
O23 Cs12 B10 85.6(5) 3_445 4_455 ?
O23 Cs12 B13 23.7(4) 3_445 3_445 ?
O23 Cs12 B17 107.7(5) 3_445 4_454 ?
O23 Cs12 B19 107.7(5) 3_445 . ?
O23 Cs12 O27 84.6(4) 3_445 2_565 ?
O23 Cs12 O39 99.9(4) 3_445 4_455 ?
O24 Cs12 Cs11 56.2(3) 3_445 . ?
O24 Cs12 B10 123.4(5) 3_445 4_455 ?
O24 Cs12 B13 21.2(4) 3_445 3_445 ?
O24 Cs12 B17 83.7(5) 3_445 4_454 ?
O24 Cs12 B19 125.6(6) 3_445 . ?
O24 Cs12 O23 43.3(4) 3_445 3_445 ?
O24 Cs12 O26 107.7(4) 3_445 4_455 ?
O24 Cs12 O27 107.3(4) 3_445 2_565 ?
O24 Cs12 O39 127.6(4) 3_445 4_455 ?
O26 Cs12 Cs11 95.4(3) 4_455 . ?
O26 Cs12 B10 20.4(5) 4_455 4_455 ?
O26 Cs12 B13 86.6(5) 4_455 3_445 ?
O26 Cs12 B17 106.9(5) 4_455 4_454 ?
O26 Cs12 B19 84.6(6) 4_455 . ?
O26 Cs12 O23 66.6(4) 4_455 3_445 ?
O26 Cs12 O27 75.7(4) 4_455 2_565 ?
O26 Cs12 O39 41.2(3) 4_455 4_455 ?
O27 Cs12 Cs11 51.3(3) 2_565 . ?
O27 Cs12 B10 84.3(4) 2_565 4_455 ?
O27 Cs12 B13 102.2(5) 2_565 3_445 ?
O27 Cs12 B17 167.6(5) 2_565 4_454 ?
O29 Cs12 Cs11 76.9(4) . . ?
O29 Cs12 B10 101.1(5) . 4_455 ?
O29 Cs12 B13 132.9(5) . 3_445 ?
O29 Cs12 B17 127.5(6) . 4_454 ?
O29 Cs12 B19 21.5(5) . . ?
O29 Cs12 O22 110.5(5) . 4_454 ?
O29 Cs12 O23 123.2(5) . 3_445 ?
O29 Cs12 O24 124.4(5) . 3_445 ?
O29 Cs12 O26 104.5(5) . 4_455 ?
O29 Cs12 O27 41.3(5) . 2_565 ?
O29 Cs12 O39 106.5(4) . 4_455 ?
O39 Cs12 Cs11 136.5(2) 4_455 . ?
O39 Cs12 B10 22.1(4) 4_455 4_455 ?
O39 Cs12 B13 111.0(5) 4_455 3_445 ?
O39 Cs12 B17 74.2(4) 4_455 4_454 ?
O39 Cs12 B19 96.9(5) 4_455 . ?
O39 Cs12 O27 102.3(3) 4_455 2_565 ?
Cs3 Zn1 Cs3 118.38(8) 3_545 4 ?
Cs3 Zn1 Cs12 105.08(8) 3_545 4 ?
Cs6 Zn1 Cs3 112.58(9) 4 3_545 ?
Cs6 Zn1 Cs3 58.21(6) 4 4 ?
Cs6 Zn1 Cs12 118.11(8) 4 4 ?
Cs11 Zn1 Cs3 104.33(9) . 3_545 ?
Cs11 Zn1 Cs3 137.29(7) . 4 ?
Cs11 Zn1 Cs6 107.04(8) . 4 ?
Cs11 Zn1 Cs12 108.84(9) . 4 ?
Cs12 Zn1 Cs3 61.06(5) 4 4 ?
O4 Zn1 Cs3 47.0(4) 4 4 ?
O4 Zn1 Cs3 78.9(4) 4 3_545 ?
O4 Zn1 Cs6 50.5(3) 4 4 ?
O4 Zn1 Cs11 154.6(4) 4 . ?
O4 Zn1 Cs12 94.2(4) 4 4 ?
O22 Zn1 Cs3 77.4(5) . 3_545 ?
O22 Zn1 Cs3 91.8(4) . 4 ?
O22 Zn1 Cs6 149.9(4) . 4 ?
O22 Zn1 Cs11 97.1(5) . . ?
O22 Zn1 Cs12 34.2(4) . 4 ?
O22 Zn1 O4 108.1(6) . 4 ?
O22 Zn1 O31 99.7(6) . 2 ?
O22 Zn1 O38 118.8(7) . . ?
O31 Zn1 Cs3 157.2(5) 2 4 ?
O31 Zn1 Cs3 47.0(4) 2 3_545 ?
O31 Zn1 Cs6 107.6(5) 2 4 ?
O31 Zn1 Cs11 60.9(4) 2 . ?
O31 Zn1 Cs12 133.8(4) 2 4 ?
O31 Zn1 O4 110.4(6) 2 4 ?
O38 Zn1 Cs3 81.1(4) . 4 ?
O38 Zn1 Cs3 155.7(4) . 3_545 ?
O38 Zn1 Cs6 63.5(5) . 4 ?
O38 Zn1 Cs11 58.1(4) . . ?
O38 Zn1 Cs12 97.0(4) . 4 ?
O38 Zn1 O4 109.7(6) . 4 ?
O38 Zn1 O31 109.6(6) . 2 ?
Cs5 Zn2 Cs6 108.73(9) 3_445 3_545 ?
Cs5 Zn2 Cs9 60.35(5) 3_445 4_454 ?
Cs5 Zn2 Cs12 98.47(8) 3_445 . ?
Cs6 Zn2 Cs9 119.66(7) 3_545 4_454 ?
Cs6 Zn2 Cs12 106.79(8) 3_545 . ?
Cs9 Zn2 Cs12 132.79(8) 4_454 . ?
Cs10 Zn2 Cs5 123.03(8) 2_564 3_445 ?
Cs10 Zn2 Cs6 107.14(9) 2_564 3_545 ?
Cs10 Zn2 Cs9 63.74(6) 2_564 4_454 ?
Cs10 Zn2 Cs12 111.57(9) 2_564 . ?
O18 Zn2 Cs5 71.5(5) 4_454 3_445 ?
O18 Zn2 Cs6 154.4(4) 4_454 3_545 ?
O18 Zn2 Cs9 37.0(5) 4_454 4_454 ?
O18 Zn2 Cs10 57.5(5) 4_454 2_564 ?
O18 Zn2 Cs12 98.4(4) 4_454 . ?
O18 Zn2 O24 126.7(7) 4_454 3_445 ?
O18 Zn2 O25 99.4(7) 4_454 . ?
O18 Zn2 O40 111.8(7) 4_454 . ?
O24 Zn2 Cs5 82.2(5) 3_445 3_445 ?
O24 Zn2 Cs6 77.7(6) 3_445 3_545 ?
O24 Zn2 Cs9 141.7(5) 3_445 4_454 ?
O24 Zn2 Cs10 148.5(5) 3_445 2_564 ?
O24 Zn2 Cs12 40.3(6) 3_445 . ?
O24 Zn2 O25 107.3(7) 3_445 . ?
O24 Zn2 O40 103.6(6) 3_445 . ?
O25 Zn2 Cs5 61.2(4) . 3_445 ?
O25 Zn2 Cs6 61.6(5) . 3_545 ?
O25 Zn2 Cs9 62.9(5) . 4_454 ?
O25 Zn2 Cs10 101.9(4) . 2_564 ?
O25 Zn2 Cs12 146.5(4) . . ?
O40 Zn2 Cs5 167.8(4) . 3_445 ?
O40 Zn2 Cs6 63.0(4) . 3_545 ?
O40 Zn2 Cs9 114.7(3) . 4_454 ?
O40 Zn2 Cs10 55.9(4) . 2_564 ?
O40 Zn2 Cs12 92.7(4) . . ?
O40 Zn2 O25 106.6(6) . . ?
Cs1 Zn3 Cs7 121.76(8) . 3_545 ?
Cs1 Zn3 Cs8 106.75(9) . 2_564 ?
Cs1 Zn3 Cs9 60.49(5) . . ?
Cs1 Zn3 Cs12 107.62(8) . 4_554 ?
Cs7 Zn3 Cs9 61.27(6) 3_545 . ?
Cs7 Zn3 Cs12 106.11(9) 3_545 4_554 ?
Cs8 Zn3 Cs7 109.01(9) 2_564 3_545 ?
Cs8 Zn3 Cs9 129.12(8) 2_564 . ?
Cs8 Zn3 Cs12 104.30(8) 2_564 4_554 ?
Cs9 Zn3 Cs12 126.58(8) . 4_554 ?
O15 Zn3 Cs1 97.9(4) . . ?
O15 Zn3 Cs7 51.9(4) . 3_545 ?
O15 Zn3 Cs8 74.6(4) . 2_564 ?
O15 Zn3 Cs9 60.7(4) . . ?
O15 Zn3 Cs12 153.4(4) . 4_554 ?
O26 Zn3 Cs1 152.4(4) . . ?
O26 Zn3 Cs7 81.0(5) . 3_545 ?
O26 Zn3 Cs8 76.3(6) . 2_564 ?
O26 Zn3 Cs9 138.8(6) . . ?
O26 Zn3 Cs12 46.7(5) . 4_554 ?
O26 Zn3 O15 109.2(6) . . ?
O26 Zn3 O37 109.2(6) . 2_564 ?
O33 Zn3 Cs1 54.8(5) . . ?
O33 Zn3 Cs7 84.6(5) . 3_545 ?
O33 Zn3 Cs8 161.5(5) . 2_564 ?
O33 Zn3 Cs9 46.3(5) . . ?
O33 Zn3 Cs12 82.9(5) . 4_554 ?
O33 Zn3 O15 106.6(6) . . ?
O33 Zn3 O26 119.2(8) . . ?
O33 Zn3 O37 106.5(6) . 2_564 ?
O37 Zn3 Cs1 56.5(3) 2_564 . ?
O37 Zn3 Cs7 157.1(4) 2_564 3_545 ?
O37 Zn3 Cs8 56.4(4) 2_564 2_564 ?
O37 Zn3 Cs9 111.9(4) 2_564 . ?
O37 Zn3 Cs12 95.3(4) 2_564 4_554 ?
O37 Zn3 O15 105.2(6) 2_564 . ?
Cs2 Zn4 Cs3 117.52(7) 2_565 . ?
Cs2 Zn4 Cs4 121.69(8) 2_565 . ?
Cs4 Zn4 Cs2 101.04(9) 2_565 2_565 ?
Cs4 Zn4 Cs3 91.38(6) . . ?
Cs4 Zn4 Cs3 57.61(5) 2_565 . ?
Cs4 Zn4 Cs4 136.17(8) 2_565 . ?
Cs8 Zn4 Cs2 116.58(9) . 2_565 ?
Cs8 Zn4 Cs3 125.84(8) . . ?
Cs8 Zn4 Cs4 109.07(10) . 2_565 ?
Cs8 Zn4 Cs4 62.11(6) . . ?
O12 Zn4 Cs2 46.0(5) 2_565 2_565 ?
O12 Zn4 Cs3 106.9(4) 2_565 . ?
O12 Zn4 Cs4 161.3(4) 2_565 . ?
O12 Zn4 Cs4 60.7(4) 2_565 2_565 ?
O12 Zn4 Cs8 108.0(4) 2_565 . ?
O12 Zn4 O16 113.1(6) 2_565 . ?
O16 Zn4 Cs2 81.8(4) . 2_565 ?
O16 Zn4 Cs3 136.7(4) . . ?
O16 Zn4 Cs4 48.2(4) . . ?
O16 Zn4 Cs4 162.0(5) . 2_565 ?
O16 Zn4 Cs8 55.0(5) . . ?
O17 Zn4 Cs2 156.6(4) . 2_565 ?
O17 Zn4 Cs3 70.0(4) . . ?
O17 Zn4 Cs4 62.9(4) . 2_565 ?
O17 Zn4 Cs4 78.4(4) . . ?
O17 Zn4 Cs8 59.4(4) . . ?
O17 Zn4 O12 111.3(6) . 2_565 ?
O17 Zn4 O16 108.3(6) . . ?
O29 Zn4 Cs2 78.8(6) . 2_565 ?
O29 Zn4 Cs3 49.2(6) . . ?
O29 Zn4 Cs4 87.0(5) . . ?
O29 Zn4 Cs4 92.6(5) . 2_565 ?
O29 Zn4 Cs8 149.1(5) . . ?
O29 Zn4 O12 101.7(7) . 2_565 ?
O29 Zn4 O16 105.4(7) . . ?
O29 Zn4 O17 116.9(8) . . ?
Cs1 B1 Cs2 116.8(6) 4_455 2_565 ?
Cs1 B1 Cs6 61.7(4) 4_455 4 ?
Cs2 B1 Cs6 152.9(6) 2_565 4 ?
O21 B1 Cs1 64.9(11) 1_556 4_455 ?
O21 B1 Cs2 120.8(14) 1_556 2_565 ?
O21 B1 Cs6 84.2(13) 1_556 4 ?
O38 B1 Cs1 58.4(11) . 4_455 ?
O38 B1 Cs2 93.5(12) . 2_565 ?
O38 B1 Cs6 61.9(12) . 4 ?
O38 B1 O21 122(2) . 1_556 ?
O38 B1 O39 118.4(17) . 1_556 ?
O39 B1 Cs1 169.2(15) 1_556 4_455 ?
O39 B1 Cs2 52.3(10) 1_556 2_565 ?
O39 B1 Cs6 127.3(13) 1_556 4 ?
O39 B1 O21 119.1(18) 1_556 1_556 ?
Cs5 B2 Cs1 66.3(4) 2_565 2_565 ?
Cs5 B2 Cs8 70.1(4) 2_565 . ?
Cs8 B2 Cs1 112.2(5) . 2_565 ?
O11 B2 Cs1 112.4(13) . 2_565 ?
O11 B2 Cs5 59.3(10) . 2_565 ?
O11 B2 Cs8 84.3(11) . . ?
O11 B2 O23 118.2(15) . . ?
O11 B2 O37 122.4(19) . . ?
O23 B2 Cs1 103.1(11) . 2_565 ?
O23 B2 Cs5 163.5(13) . 2_565 ?
O23 B2 Cs8 126.3(13) . . ?
O37 B2 Cs1 54.1(9) . 2_565 ?
O37 B2 Cs5 65.8(11) . 2_565 ?
O37 B2 Cs8 61.6(10) . . ?
O37 B2 O23 119.3(18) . . ?
Cs9 B3 Cs5 69.6(4) . 2_565 ?
O13 B3 Cs5 59.4(12) . 2_565 ?
O13 B3 Cs9 75.7(11) . . ?
O13 B3 O28 117(2) . . ?
O18 B3 Cs5 81.0(14) . 2_565 ?
O18 B3 Cs9 55.1(11) . . ?
O18 B3 O13 126(2) . . ?
O18 B3 O28 117(2) . . ?
O28 B3 Cs5 136.9(16) . 2_565 ?
O28 B3 Cs9 153.4(17) . . ?
Cs6 B4 Cs10 106.8(6) 3_545 2_564 ?
Cs6 B4 Cs11 66.6(5) 3_545 . ?
Cs7 B4 Cs6 68.5(5) 3_545 3_545 ?
Cs7 B4 Cs10 63.5(4) 3_545 2_564 ?
Cs7 B4 Cs11 129.6(8) 3_545 . ?
Cs11 B4 Cs10 152.7(6) . 2_564 ?
O6 B4 Cs6 55.9(13) . 3_545 ?
O6 B4 Cs7 74.5(11) . 3_545 ?
O6 B4 Cs10 137.9(13) . 2_564 ?
O6 B4 Cs11 62.1(10) . . ?
O6 B4 O20 118.3(19) . . ?
O20 B4 Cs6 159.8(13) . 3_545 ?
O20 B4 Cs7 130.9(14) . 3_545 ?
O20 B4 Cs10 89.7(12) . 2_564 ?
O20 B4 Cs11 93.5(11) . . ?
O40 B4 Cs6 69.2(14) . 3_545 ?
O40 B4 Cs7 67.7(11) . 3_545 ?
O40 B4 Cs10 43.2(11) . 2_564 ?
O40 B4 Cs11 114.2(14) . . ?
O40 B4 O6 122(2) . . ?
O40 B4 O20 120(2) . . ?
Cs7 B5 Cs9 124.5(6) 3_545 4_454 ?
Cs10 B5 Cs7 63.4(4) 2_564 3_545 ?
Cs10 B5 Cs9 69.3(4) 2_564 4_454 ?
O2 B5 Cs7 51.2(9) . 3_545 ?
O2 B5 Cs9 116.2(13) . 4_454 ?
O2 B5 Cs10 53.6(9) . 2_564 ?
O2 B5 O21 109.8(18) . . ?
O7 B5 Cs7 80.1(11) . 3_545 ?
O7 B5 Cs9 134.4(14) . 4_454 ?
O7 B5 Cs10 142.7(13) . 2_564 ?
O7 B5 O2 109.1(17) . . ?
O7 B5 O10 110.3(18) . . ?
O7 B5 O21 106.8(17) . . ?
O10 B5 Cs7 81.4(10) . 3_545 ?
O10 B5 Cs9 49.4(9) . 4_454 ?
O10 B5 Cs10 59.2(10) . 2_564 ?
O10 B5 O2 109.1(16) . . ?
O10 B5 O21 111.8(16) . . ?
O21 B5 Cs7 160.7(14) . 3_545 ?
O21 B5 Cs9 63.6(9) . 4_454 ?
O21 B5 Cs10 110.2(13) . 2_564 ?
Cs5 B6 Cs1 65.0(3) . . ?
O1 B6 Cs1 53.0(8) . . ?
O1 B6 Cs5 54.2(8) . . ?
O9 B6 Cs1 57.0(8) . . ?
O9 B6 Cs5 86.9(10) . . ?
O9 B6 O1 108.9(14) . . ?
O9 B6 O11 110.6(17) . . ?
O11 B6 Cs1 116.3(13) . . ?
O11 B6 Cs5 160.4(14) . . ?
O11 B6 O1 109.5(16) . . ?
O14 B6 Cs1 136.0(12) . . ?
O14 B6 Cs5 72.0(10) . . ?
O14 B6 O1 107.3(17) . . ?
O14 B6 O9 113.3(17) . . ?
O14 B6 O11 107.2(15) . . ?
Cs3 B7 Cs11 116.3(7) 4_554 2_554 ?
Cs6 B7 Cs3 70.1(4) 4_554 4_554 ?
Cs6 B7 Cs11 67.9(5) 4_554 2_554 ?
O7 B7 Cs3 56.0(10) . 4_554 ?
O7 B7 Cs6 86.9(12) . 4_554 ?
O7 B7 Cs11 154.1(15) . 2_554 ?
O31 B7 Cs3 66.6(11) . 4_554 ?
O31 B7 Cs6 64.4(11) . 4_554 ?
O31 B7 Cs11 52.9(12) . 2_554 ?
O31 B7 O7 121.8(18) . . ?
O31 B7 O35 121(2) . . ?
O35 B7 Cs3 166.3(17) . 4_554 ?
O35 B7 Cs6 123.0(15) . 4_554 ?
O35 B7 Cs11 75.3(13) . 2_554 ?
O35 B7 O7 117(2) . . ?
Cs2 B8 Cs5 76.4(5) . . ?
Cs2 B8 Cs8 67.7(5) . . ?
Cs8 B8 Cs5 135.5(7) . . ?
O12 B8 Cs2 61.3(12) . . ?
O12 B8 Cs5 116.6(15) . . ?
O12 B8 Cs8 67.6(10) . . ?
O12 B8 O30 122(2) . . ?
O14 B8 Cs2 58.4(11) . . ?
O14 B8 Cs5 61.1(11) . . ?
O14 B8 Cs8 77.6(12) . . ?
O14 B8 O12 118(2) . . ?
O14 B8 O30 119.8(19) . . ?
O30 B8 Cs2 167.7(16) . . ?
O30 B8 Cs5 92.1(13) . . ?
O30 B8 Cs8 124.5(16) . . ?
Cs3 B9 Cs3 152.4(7) . 2_564 ?
Cs7 B9 Cs3 114.7(6) . . ?
Cs7 B9 Cs3 82.7(5) . 2_564 ?
O4 B9 Cs3 94.7(11) . 2_564 ?
O4 B9 Cs3 67.7(10) . . ?
O4 B9 Cs7 84.2(13) . . ?
O4 B9 O19 120.6(18) . . ?
O4 B9 O32 122.4(19) . . ?
O19 B9 Cs3 130.9(13) . 2_564 ?
O19 B9 Cs3 54.6(9) . . ?
O19 B9 Cs7 129.9(14) . . ?
O32 B9 Cs3 162.0(14) . . ?
O32 B9 Cs3 45.6(9) . 2_564 ?
O32 B9 Cs7 56.2(11) . . ?
O32 B9 O19 117.0(17) . . ?
Cs2 B10 Cs7 155.6(8) 2_564 3_545 ?
Cs2 B10 Cs10 103.9(7) 2_564 2_564 ?
Cs2 B10 Cs12 68.7(4) 2_564 4_554 ?
Cs7 B10 Cs10 59.6(3) 3_545 2_564 ?
Cs12 B10 Cs7 116.9(6) 4_554 3_545 ?
Cs12 B10 Cs10 153.0(8) 4_554 2_564 ?
O2 B10 Cs2 135.5(15) . 2_564 ?
O2 B10 Cs7 43.4(9) . 3_545 ?
O2 B10 Cs10 40.6(11) . 2_564 ?
O2 B10 Cs12 155.7(16) . 4_554 ?
O2 B10 O39 118(2) . . ?
O26 B10 Cs2 74.2(13) . 2_564 ?
O26 B10 Cs7 89.1(12) . 3_545 ?
O26 B10 Cs10 96.4(14) . 2_564 ?
O26 B10 Cs12 56.8(11) . 4_554 ?
O26 B10 O2 124.2(18) . . ?
O26 B10 O39 117.8(19) . . ?
O39 B10 Cs2 61.6(11) . 2_564 ?
O39 B10 Cs7 142.7(17) . 3_545 ?
O39 B10 Cs10 133.7(14) . 2_564 ?
O39 B10 Cs12 67.2(11) . 4_554 ?
Cs2 B11 Cs5 76.7(5) 2_565 2_565 ?
Cs2 B11 Cs11 65.5(3) 2_565 . ?
Cs11 B11 Cs5 136.5(6) . 2_565 ?
O3 B11 Cs2 53.6(8) . 2_565 ?
O3 B11 Cs5 52.9(9) . 2_565 ?
O3 B11 Cs11 86.4(10) . . ?
O3 B11 O6 110.0(15) . . ?
O3 B11 O13 108.1(17) . . ?
O6 B11 Cs2 132.8(12) . 2_565 ?
O6 B11 Cs5 133.1(12) . 2_565 ?
O6 B11 Cs11 69.9(10) . . ?
O8 B11 Cs2 56.6(9) . 2_565 ?
O8 B11 Cs5 118.9(12) . 2_565 ?
O8 B11 Cs11 55.4(9) . . ?
O8 B11 O3 109.3(15) . . ?
O8 B11 O6 107.9(17) . . ?
O8 B11 O13 110.4(15) . . ?
O13 B11 Cs2 116.2(12) . 2_565 ?
O13 B11 Cs5 55.7(10) . 2_565 ?
O13 B11 Cs11 163.3(14) . . ?
O13 B11 O6 111.0(16) . . ?
Cs3 B12 Cs4 63.2(4) 2_564 . ?
Cs7 B12 Cs3 83.9(5) . 2_564 ?
Cs7 B12 Cs4 134.1(7) . . ?
O5 B12 Cs3 109.1(13) . 2_564 ?
O5 B12 Cs4 161.2(13) . . ?
O5 B12 Cs7 56.8(10) . . ?
O5 B12 O32 108.8(17) . . ?
O5 B12 O36 109.9(16) . . ?
O32 B12 Cs3 54.9(9) . 2_564 ?
O32 B12 Cs4 81.3(12) . . ?
O32 B12 Cs7 53.0(10) . . ?
O32 B12 O36 103.5(17) . . ?
O34 B12 Cs3 137.1(16) . 2_564 ?
O34 B12 Cs4 74.8(13) . . ?
O34 B12 Cs7 123.2(14) . . ?
O34 B12 O5 114(2) . . ?
O34 B12 O32 112.3(17) . . ?
O34 B12 O36 108.1(18) . . ?
O36 B12 Cs3 51.0(9) . 2_564 ?
O36 B12 Cs4 51.5(10) . . ?
O36 B12 Cs7 128.2(13) . . ?
Cs11 B13 Cs5 158.9(7) 3 . ?
Cs12 B13 Cs5 113.2(7) 3 . ?
Cs12 B13 Cs11 68.2(5) 3 3 ?
O1 B13 Cs5 46.2(9) . . ?
O1 B13 Cs11 139.0(16) . 3 ?
O1 B13 Cs12 151.5(15) . 3 ?
O1 B13 O23 116.4(19) . . ?
O23 B13 Cs5 139.8(13) . . ?
O23 B13 Cs11 60.9(10) . 3 ?
O23 B13 Cs12 63.9(12) . 3 ?
O24 B13 Cs5 89.8(13) . . ?
O24 B13 Cs11 72.7(13) . 3 ?
O24 B13 Cs12 58.8(13) . 3 ?
O24 B13 O1 127.7(19) . . ?
O24 B13 O23 116(2) . . ?
Cs8 B14 Cs10 61.0(4) 2_564 2_564 ?
Cs9 B14 Cs8 144.9(7) . 2_564 ?
Cs9 B14 Cs10 119.5(8) . 2_564 ?
O9 B14 Cs8 126.6(14) . 2_564 ?
O9 B14 Cs9 54.7(11) . . ?
O9 B14 Cs10 172.4(15) . 2_564 ?
O15 B14 Cs8 77.9(12) . 2_564 ?
O15 B14 Cs9 76.4(14) . . ?
O15 B14 Cs10 55.6(12) . 2_564 ?
O15 B14 O9 123(2) . . ?
O15 B14 O30 118(2) . . ?
O30 B14 Cs8 66.4(12) . 2_564 ?
O30 B14 Cs9 148.1(14) . . ?
O30 B14 Cs10 62.9(13) . 2_564 ?
O30 B14 O9 119(2) . . ?
Cs8 B15 Cs4 69.5(4) . . ?
Cs8 B15 Cs10 67.1(4) . . ?
Cs10 B15 Cs4 136.1(7) . . ?
O17 B15 Cs4 106.7(13) . . ?
O17 B15 Cs8 63.7(11) . . ?
O17 B15 Cs10 58.9(11) . . ?
O19 B15 Cs4 80.8(12) . . ?
O19 B15 Cs8 148.4(15) . . ?
O19 B15 Cs10 143.1(15) . . ?
O19 B15 O17 117.5(19) . . ?
O34 B15 Cs4 80.4(13) . . ?
O34 B15 Cs8 63.8(12) . . ?
O34 B15 Cs10 74.9(12) . . ?
O34 B15 O17 120(2) . . ?
O34 B15 O19 123(2) . . ?
Cs4 B16 Cs2 148.3(6) . 2_565 ?
Cs5 B16 Cs2 75.6(4) 2_565 2_565 ?
Cs5 B16 Cs4 121.7(7) 2_565 . ?
O3 B16 Cs2 39.8(9) . 2_565 ?
O3 B16 Cs4 170.1(14) . . ?
O3 B16 Cs5 60.8(11) . 2_565 ?
O3 B16 O20 116.5(19) . . ?
O16 B16 Cs2 96.0(12) . 2_565 ?
O16 B16 Cs4 64.3(11) . . ?
O16 B16 Cs5 81.4(13) . 2_565 ?
O16 B16 O3 125(2) . . ?
O16 B16 O20 118.4(19) . . ?
O20 B16 Cs2 133.6(15) . 2_565 ?
O20 B16 Cs4 54.4(10) . . ?
O20 B16 Cs5 135.8(13) . 2_565 ?
Cs12 B17 Cs2 69.2(4) 4 2_565 ?
O8 B17 Cs2 54.0(11) . 2_565 ?
O8 B17 Cs12 123.1(14) . 4 ?
O8 B17 O28 117(2) . . ?
O22 B17 Cs2 92.7(14) . 2_565 ?
O22 B17 Cs12 52.9(11) . 4 ?
O22 B17 O8 127(2) . . ?
O22 B17 O28 116(2) . . ?
O28 B17 Cs2 124.4(17) . 2_565 ?
O28 B17 Cs12 90.6(13) . 4 ?
Cs6 B18 Cs1 63.0(4) 3_545 3_445 ?
Cs9 B18 Cs1 115.2(7) 4_454 3_445 ?
Cs9 B18 Cs6 152.7(7) 4_454 3_545 ?
O10 B18 Cs1 170.5(15) . 3_445 ?
O10 B18 Cs6 125.3(15) . 3_545 ?
O10 B18 Cs9 55.2(10) . 4_454 ?
O10 B18 O35 119.4(18) . . ?
O25 B18 Cs1 52.8(12) . 3_445 ?
O25 B18 Cs6 68.4(12) . 3_545 ?
O25 B18 Cs9 88.7(13) . 4_454 ?
O25 B18 O10 123(2) . . ?
O25 B18 O35 117(2) . . ?
O35 B18 Cs1 64.8(12) . 3_445 ?
O35 B18 Cs6 78.7(13) . 3_545 ?
O35 B18 Cs9 126.7(15) . 4_454 ?
Cs3 B19 Cs2 159.7(9) . 2_565 ?
Cs3 B19 Cs12 78.1(5) . . ?
Cs12 B19 Cs2 111.1(7) . 2_565 ?
O27 B19 Cs2 66.8(12) 2_565 2_565 ?
O27 B19 Cs3 133.5(16) 2_565 . ?
O27 B19 Cs12 78.7(14) 2_565 . ?
O29 B19 Cs2 92.4(15) . 2_565 ?
O29 B19 Cs3 78.3(15) . . ?
O29 B19 Cs12 53.7(12) . . ?
O29 B19 O27 117(2) . 2_565 ?
O29 B19 O36 123(2) . 2_565 ?
O36 B19 Cs2 112.1(14) 2_565 2_565 ?
O36 B19 Cs3 60.9(12) 2_565 . ?
O36 B19 Cs12 136.8(16) 2_565 . ?
O36 B19 O27 119(2) 2_565 2_565 ?
Cs9 B20 Cs7 65.8(5) . 3_545 ?
O5 B20 Cs7 43.1(11) 3_545 3_545 ?
O5 B20 Cs9 68.0(12) 3_545 . ?
O5 B20 O27 119(2) 3_545 3_545 ?
O27 B20 Cs7 141.0(17) 3_545 3_545 ?
O27 B20 Cs9 149.9(17) 3_545 . ?
O33 B20 Cs7 89.0(15) . 3_545 ?
O33 B20 Cs9 62.2(13) . . ?
O33 B20 O5 122(2) . 3_545 ?
O33 B20 O27 119(2) . 3_545 ?
Cs5 O1 Cs1 81.2(3) . . ?
B6 O1 Cs1 103.8(11) . . ?
B6 O1 Cs5 101.7(10) . . ?
B13 O1 Cs1 126.0(13) . . ?
B13 O1 Cs5 114.4(13) . . ?
B13 O1 B6 120.8(15) . . ?
Cs7 O2 Cs10 79.7(3) 3_545 2_564 ?
B5 O2 Cs7 106.3(11) . 3_545 ?
B5 O2 Cs10 103.6(11) . 2_564 ?
B10 O2 Cs7 118.4(12) . 3_545 ?
B10 O2 Cs10 122.6(14) . 2_564 ?
B10 O2 B5 119.0(16) . . ?
Cs2 O3 Cs5 97.5(4) 2_565 2_565 ?
B11 O3 Cs2 103.4(10) . 2_565 ?
B11 O3 Cs5 104.4(11) . 2_565 ?
B16 O3 Cs2 123.3(11) . 2_565 ?
B16 O3 Cs5 96.0(12) . 2_565 ?
B16 O3 B11 125.6(16) . . ?
Cs3 O4 Cs7 118.6(4) . . ?
Cs6 O4 Cs3 78.4(3) . . ?
Cs6 O4 Cs7 72.9(3) . . ?
Zn1 O4 Cs3 107.1(5) 4_454 . ?
Zn1 O4 Cs6 98.8(4) 4_454 . ?
Zn1 O4 Cs7 130.0(5) 4_454 . ?
B9 O4 Cs3 90.2(11) . . ?
B9 O4 Cs6 134.0(12) . . ?
B9 O4 Cs7 74.2(12) . . ?
B9 O4 Zn1 127.0(12) . 4_454 ?
Cs7 O5 Cs9 79.8(3) . 3_455 ?
B12 O5 Cs7 100.3(11) . . ?
B12 O5 Cs9 138.6(12) . 3_455 ?
B20 O5 Cs7 119.2(14) 3_455 . ?
B20 O5 Cs9 88.5(14) 3_455 3_455 ?
B20 O5 B12 124.5(18) 3_455 . ?
Cs6 O6 Cs7 76.4(3) 3_545 3_545 ?
Cs6 O6 Cs11 78.1(3) 3_545 . ?
Cs7 O6 Cs11 153.8(5) 3_545 . ?
B4 O6 Cs6 102.3(14) . 3_545 ?
B4 O6 Cs7 82.2(11) . 3_545 ?
B4 O6 Cs11 97.3(11) . . ?
B4 O6 B11 123.8(18) . . ?
B11 O6 Cs6 132.8(12) . 3_545 ?
B11 O6 Cs7 115.8(10) . 3_545 ?
B11 O6 Cs11 86.3(10) . . ?
Cs3 O7 Cs6 73.5(3) 4_554 4_554 ?
Cs3 O7 Cs7 95.1(4) 4_554 3_545 ?
Cs6 O7 Cs7 167.0(5) 4_554 3_545 ?
B5 O7 Cs3 134.7(12) . 4_554 ?
B5 O7 Cs6 115.1(12) . 4_554 ?
B5 O7 Cs7 77.2(11) . 3_545 ?
B7 O7 Cs3 101.2(12) . 4_554 ?
B7 O7 Cs6 71.0(12) . 4_554 ?
B7 O7 Cs7 106.2(13) . 3_545 ?
B7 O7 B5 123.9(17) . . ?
Cs11 O8 Cs2 79.6(3) . 2_565 ?
B11 O8 Cs2 100.2(11) . 2_565 ?
B11 O8 Cs11 101.5(10) . . ?
B17 O8 Cs2 105.2(12) . 2_565 ?
B17 O8 Cs11 129.3(13) . . ?
B17 O8 B11 126.0(16) . . ?
Cs1 O9 Cs5 67.8(2) . . ?
Cs9 O9 Cs1 78.6(3) . . ?
Cs9 O9 Cs5 146.3(4) . . ?
B6 O9 Cs1 100.2(10) . . ?
B6 O9 Cs5 70.7(10) . . ?
B6 O9 Cs9 120.4(11) . . ?
B14 O9 Cs1 124.8(12) . . ?
B14 O9 Cs5 93.5(13) . . ?
B14 O9 Cs9 103.3(14) . . ?
B14 O9 B6 122.6(17) . . ?
Cs9 O10 Cs7 153.0(5) 4_454 3_545 ?
Cs9 O10 Cs10 85.9(3) 4_454 2_564 ?
Cs10 O10 Cs7 67.2(2) 2_564 3_545 ?
B5 O10 Cs7 76.0(10) . 3_545 ?
B5 O10 Cs9 109.0(11) . 4_454 ?
B5 O10 Cs10 97.6(12) . 2_564 ?
B18 O10 Cs7 95.5(12) . 3_545 ?
B18 O10 Cs9 102.9(12) . 4_454 ?
B18 O10 Cs10 131.5(12) . 2_564 ?
B18 O10 B5 122.7(17) . . ?
Cs5 O11 Cs8 73.6(3) 2_565 . ?
B2 O11 Cs5 98.4(10) . 2_565 ?
B2 O11 Cs8 74.6(11) . . ?
B2 O11 B6 116.8(16) . . ?
B6 O11 Cs5 142.3(12) . 2_565 ?
B6 O11 Cs8 101.8(11) . . ?
Cs2 O12 Cs4 144.3(5) . . ?
Cs2 O12 Cs8 76.2(3) . . ?
Cs8 O12 Cs4 77.3(3) . . ?
Zn4 O12 Cs2 107.2(6) 2_564 . ?
Zn4 O12 Cs4 89.5(5) 2_564 . ?
Zn4 O12 Cs8 158.3(6) 2_564 . ?
B8 O12 Cs2 95.8(13) . . ?
B8 O12 Cs4 107.5(14) . . ?
B8 O12 Cs8 89.4(11) . . ?
B8 O12 Zn4 111.1(13) . 2_564 ?
Cs5 O13 Cs9 76.1(3) 2_565 . ?
B3 O13 Cs5 99.1(13) . 2_565 ?
B3 O13 Cs9 82.3(12) . . ?
B3 O13 B11 124.6(16) . . ?
B11 O13 Cs5 101.3(12) . 2_565 ?
B11 O13 Cs9 152.8(11) . . ?
Cs2 O14 Cs5 90.0(4) . . ?
Cs2 O14 Cs8 73.5(3) . . ?
Cs5 O14 Cs8 162.9(5) . . ?
B6 O14 Cs2 139.6(12) . . ?
B6 O14 Cs5 84.2(10) . . ?
B6 O14 Cs8 111.3(10) . . ?
B8 O14 Cs2 99.1(13) . . ?
B8 O14 Cs5 98.5(12) . . ?
B8 O14 Cs8 80.0(11) . . ?
B8 O14 B6 121.3(18) . . ?
Cs7 O15 Cs8 130.8(4) 3_545 2_564 ?
Cs7 O15 Cs9 75.0(3) 3_545 . ?
Cs7 O15 Cs10 74.8(3) 3_545 2_564 ?
Cs9 O15 Cs8 151.4(4) . 2_564 ?
Cs10 O15 Cs8 66.5(3) 2_564 2_564 ?
Cs10 O15 Cs9 141.2(4) 2_564 . ?
Zn3 O15 Cs7 97.9(5) . 3_545 ?
Zn3 O15 Cs8 75.5(4) . 2_564 ?
Zn3 O15 Cs9 90.4(5) . . ?
Zn3 O15 Cs10 117.4(6) . 2_564 ?
B14 O15 Cs7 138.4(13) . 3_545 ?
B14 O15 Cs8 82.2(13) . 2_564 ?
B14 O15 Cs9 82.4(13) . . ?
B14 O15 Cs10 105.2(14) . 2_564 ?
B14 O15 Zn3 116.9(14) . . ?
Cs4 O16 Cs5 131.5(4) . 2_565 ?
Cs8 O16 Cs4 81.5(3) . . ?
Cs8 O16 Cs5 76.1(3) . 2_565 ?
Zn4 O16 Cs4 105.8(5) . . ?
Zn4 O16 Cs5 117.6(6) . 2_565 ?
Zn4 O16 Cs8 92.7(5) . . ?
B16 O16 Cs4 94.9(13) . . ?
B16 O16 Cs5 76.8(12) . 2_565 ?
B16 O16 Cs8 139.7(13) . . ?
B16 O16 Zn4 126.4(14) . . ?
Cs8 O17 Cs4 136.7(4) . 2_565 ?
Cs10 O17 Cs4 75.1(3) . 2_565 ?
Cs10 O17 Cs8 77.6(3) . . ?
Zn4 O17 Cs4 87.6(5) . 2_565 ?
Zn4 O17 Cs8 89.1(5) . . ?
Zn4 O17 Cs10 135.7(6) . . ?
B15 O17 Cs4 123.2(12) . 2_565 ?
B15 O17 Cs8 93.5(12) . . ?
B15 O17 Cs10 98.6(13) . . ?
B15 O17 Zn4 124.5(14) . . ?
Cs9 O18 Cs5 75.2(4) . 2_565 ?
Cs9 O18 Cs10 88.1(4) . 3_545 ?
Cs10 O18 Cs5 151.7(5) 3_545 2_565 ?
Zn2 O18 Cs5 78.2(6) 4 2_565 ?
Zn2 O18 Cs9 120.1(7) 4 . ?
Zn2 O18 Cs10 91.3(5) 4 3_545 ?
B3 O18 Cs5 78.0(14) . 2_565 ?
B3 O18 Cs9 103.8(13) . . ?
B3 O18 Cs10 128.9(16) . 3_545 ?
B3 O18 Zn2 121.6(14) . 4 ?
B9 O19 Cs3 102.8(11) . . ?
B15 O19 Cs3 128.7(13) . . ?
B15 O19 B9 120.4(16) . . ?
B4 O20 Cs4 132.3(12) . . ?
B16 O20 Cs4 103.9(13) . . ?
B16 O20 B4 122.1(17) . . ?
Cs1 O21 Cs9 73.1(3) 4_454 4_454 ?
B1 O21 Cs1 92.0(12) 1_554 4_454 ?
B1 O21 Cs9 148.8(12) 1_554 4_454 ?
B1 O21 B5 112.3(15) 1_554 . ?
B5 O21 Cs1 147.0(12) . 4_454 ?
B5 O21 Cs9 93.4(10) . 4_454 ?
Zn1 O22 Cs12 124.4(7) . 4 ?
B17 O22 Cs12 106.3(13) . 4 ?
B17 O22 Zn1 119.8(14) . . ?
Cs11 O23 Cs12 78.2(3) 3 3 ?
B2 O23 Cs11 117.2(11) . 3 ?
B2 O23 Cs12 139.7(11) . 3 ?
B13 O23 Cs11 95.8(11) . 3 ?
B13 O23 Cs12 92.3(13) . 3 ?
B13 O23 B2 120.4(16) . . ?
Cs12 O24 Cs11 75.5(3) 3 3 ?
Zn2 O24 Cs11 126.5(7) 3 3 ?
Zn2 O24 Cs12 116.2(8) 3 3 ?
B13 O24 Cs11 86.1(13) . 3 ?
B13 O24 Cs12 100.1(14) . 3 ?
B13 O24 Zn2 135.2(15) . 3 ?
Cs1 O25 Cs5 76.2(3) 3_445 3_445 ?
Cs1 O25 Cs6 72.7(4) 3_445 3_545 ?
Cs5 O25 Cs6 135.2(4) 3_445 3_545 ?
Zn2 O25 Cs1 128.5(6) . 3_445 ?
Zn2 O25 Cs5 87.3(5) . 3_445 ?
Zn2 O25 Cs6 87.5(5) . 3_545 ?
B18 O25 Cs1 106.7(15) . 3_445 ?
B18 O25 Cs5 130.4(14) . 3_445 ?
B18 O25 Cs6 89.6(13) . 3_545 ?
B18 O25 Zn2 120.6(15) . . ?
Cs12 O26 Cs2 76.2(3) 4_554 2_564 ?
Zn3 O26 Cs2 126.6(8) . 2_564 ?
Zn3 O26 Cs12 106.9(6) . 4_554 ?
B10 O26 Cs2 84.3(13) . 2_564 ?
B10 O26 Cs12 102.8(13) . 4_554 ?
B10 O26 Zn3 141.2(14) . . ?
Cs11 O27 Cs2 70.0(3) 2_564 . ?
Cs11 O27 Cs12 72.8(3) 2_564 2_564 ?
Cs12 O27 Cs2 118.8(4) 2_564 . ?
B19 O27 Cs2 92.1(14) 2_564 . ?
B19 O27 Cs11 131.4(14) 2_564 2_564 ?
B19 O27 Cs12 78.1(13) 2_564 2_564 ?
B20 O27 Cs2 128.9(15) 3_455 . ?
B20 O27 Cs11 109.6(15) 3_455 2_564 ?
B20 O27 Cs12 108.5(14) 3_455 2_564 ?
B20 O27 B19 116.3(19) 3_455 2_564 ?
B3 O28 Cs4 128.7(14) . 4 ?
B17 O28 Cs4 111.2(14) . 4 ?
B17 O28 B3 120(2) . . ?
Cs12 O29 Cs3 86.6(4) . . ?
Zn4 O29 Cs3 106.3(8) . . ?
Zn4 O29 Cs12 136.6(7) . . ?
B19 O29 Cs3 79.6(15) . . ?
B19 O29 Cs12 104.8(15) . . ?
B19 O29 Zn4 118.1(15) . . ?
Cs10 O30 Cs8 68.0(3) 2_564 2_564 ?
B8 O30 Cs8 111.2(14) . 2_564 ?
B8 O30 Cs10 141.1(13) . 2_564 ?
B14 O30 Cs8 92.8(12) . 2_564 ?
B14 O30 Cs10 96.6(15) . 2_564 ?
B14 O30 B8 122(2) . . ?
Cs3 O31 Cs11 152.0(5) 4_554 2_554 ?
Cs6 O31 Cs3 78.2(3) 4_554 4_554 ?
Cs6 O31 Cs11 80.3(3) 4_554 2_554 ?
Zn1 O31 Cs3 106.4(6) 2_554 4_554 ?
Zn1 O31 Cs6 157.4(7) 2_554 4_554 ?
Zn1 O31 Cs11 87.3(5) 2_554 2_554 ?
B7 O31 Cs3 90.9(12) . 4_554 ?
B7 O31 Cs6 92.8(11) . 4_554 ?
B7 O31 Cs11 108.0(13) . 2_554 ?
B7 O31 Zn1 109.0(12) . 2_554 ?
Cs7 O32 Cs3 107.4(4) . 2_564 ?
B9 O32 Cs3 116.5(12) . 2_564 ?
B9 O32 Cs7 101.4(12) . . ?
B9 O32 B12 124.0(16) . . ?
B12 O32 Cs3 102.4(11) . 2_564 ?
B12 O32 Cs7 103.5(13) . . ?
Cs1 O33 Cs9 80.1(4) . . ?
Cs1 O33 Cs11 69.4(3) . 4_554 ?
Cs9 O33 Cs11 134.9(5) . 4_554 ?
Zn3 O33 Cs1 93.9(6) . . ?
Zn3 O33 Cs9 106.8(6) . . ?
Zn3 O33 Cs11 107.6(6) . 4_554 ?
B20 O33 Cs1 145.1(15) . . ?
B20 O33 Cs9 95.1(14) . . ?
B20 O33 Cs11 92.0(14) . 4_554 ?
B20 O33 Zn3 120.3(15) . . ?
Cs8 O34 Cs4 73.0(4) . . ?
Cs8 O34 Cs10 72.3(3) . . ?
Cs10 O34 Cs4 139.7(4) . . ?
B12 O34 Cs4 83.8(13) . . ?
B12 O34 Cs8 131.6(12) . . ?
B12 O34 Cs10 135.5(14) . . ?
B15 O34 Cs4 79.5(13) . . ?
B15 O34 Cs8 94.2(13) . . ?
B15 O34 Cs10 83.2(12) . . ?
B15 O34 B12 122.9(18) . . ?
Cs1 O35 Cs6 66.5(3) 3_445 3_545 ?
Cs1 O35 Cs11 65.6(3) 3_445 2_554 ?
Cs6 O35 Cs11 111.1(4) 3_545 2_554 ?
B7 O35 Cs1 144.5(14) . 3_445 ?
B7 O35 Cs6 111.9(13) . 3_545 ?
B7 O35 Cs11 84.1(13) . 2_554 ?
B18 O35 Cs1 93.2(12) . 3_445 ?
B18 O35 Cs6 79.2(12) . 3_545 ?
B18 O35 Cs11 147.4(15) . 2_554 ?
B18 O35 B7 121.9(19) . . ?
Cs3 O36 Cs4 80.2(4) 2_564 . ?
B12 O36 Cs3 106.1(11) . 2_564 ?
B12 O36 Cs4 106.6(12) . . ?
B19 O36 Cs3 96.4(13) 2_564 2_564 ?
B19 O36 Cs4 129.8(14) 2_564 . ?
B19 O36 B12 122.1(19) 2_564 . ?
Cs1 O37 Cs5 77.4(3) 2_565 2_565 ?
Cs1 O37 Cs8 148.5(5) 2_565 . ?
Cs8 O37 Cs5 79.5(3) . 2_565 ?
Zn3 O37 Cs1 91.4(4) 2_565 2_565 ?
Zn3 O37 Cs5 140.0(5) 2_565 2_565 ?
Zn3 O37 Cs8 92.6(4) 2_565 . ?
B2 O37 Cs1 105.3(11) . 2_565 ?
B2 O37 Cs5 91.6(12) . 2_565 ?
B2 O37 Cs8 96.5(11) . . ?
B2 O37 Zn3 128.4(14) . 2_565 ?
Cs1 O38 Cs6 71.5(3) 4_455 4 ?
Cs1 O38 Cs11 77.2(3) 4_455 . ?
Cs11 O38 Cs6 134.1(4) . 4 ?
Zn1 O38 Cs1 131.9(6) . 4_455 ?
Zn1 O38 Cs6 86.3(5) . 4 ?
Zn1 O38 Cs11 90.7(5) . . ?
B1 O38 Cs1 99.7(12) . 4_455 ?
B1 O38 Cs6 98.0(13) . 4 ?
B1 O38 Cs11 119.9(13) . . ?
B1 O38 Zn1 125.9(13) . . ?
Cs2 O39 Cs3 151.9(4) 2_564 4_554 ?
Cs2 O39 Cs12 77.2(3) 2_564 4_554 ?
Cs12 O39 Cs3 75.4(3) 4_554 4_554 ?
B1 O39 Cs2 107.6(12) 1_554 2_564 ?
B1 O39 Cs3 91.9(12) 1_554 4_554 ?
B1 O39 Cs12 146.3(12) 1_554 4_554 ?
B1 O39 B10 121.1(16) 1_554 . ?
B10 O39 Cs2 95.9(14) . 2_564 ?
B10 O39 Cs3 90.8(13) . 4_554 ?
B10 O39 Cs12 90.7(12) . 4_554 ?
Cs7 O40 Cs6 74.4(3) 3_545 3_545 ?
Cs10 O40 Cs6 138.2(4) 2_564 3_545 ?
Cs10 O40 Cs7 76.6(3) 2_564 3_545 ?
Zn2 O40 Cs6 86.5(5) . 3_545 ?
Zn2 O40 Cs7 134.1(6) . 3_545 ?
Zn2 O40 Cs10 92.8(4) . 2_564 ?
B4 O40 Cs6 89.6(15) . 3_545 ?
B4 O40 Cs7 89.9(12) . 3_545 ?
B4 O40 Cs10 119.9(14) . 2_564 ?
B4 O40 Zn2 132.0(12) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
